#------------------------------------------------------------------------------
#$Date: 2016-02-20 00:18:51 +0200 (Sat, 20 Feb 2016) $
#$Revision: 176760 $
#$URL: svn://www.crystallography.net/cod/cif/2/01/26/2012637.cif $
#------------------------------------------------------------------------------
#
# This file is available in the Crystallography Open Database (COD),
# http://www.crystallography.net/. The original data for this entry
# were provided by IUCr Journals, http://journals.iucr.org/.
#
# The file may be used within the scientific community so long as
# proper attribution is given to the journal article from which the
# data were obtained.
#
data_2012637
loop_
_publ_author_name
'Yamane, Hisanori'
'Sasaki, Shinya'
'Kubota, Shunichi'
'Kajiwara, Takashi'
'Shimada, Masahiko'
_publ_section_title
;
 Ba₁₄Cu₂In₄N₇, a new subnitride with isolated nitridocuprate
 groups and indium clusters
;
_journal_issue                   4
_journal_name_full               'Acta Crystallographica Section C'
_journal_page_first              i50
_journal_page_last               i52
_journal_paper_doi               10.1107/S010827010200361X
_journal_volume                  58
_journal_year                    2002
_chemical_formula_moiety         'Ba14 Cu2 In4 N7'
_chemical_formula_structural     'Ba Ba27 N6 (Cu N2)4 (In4)2'
_chemical_formula_sum            'Ba14 Cu2 In4 N7'
_chemical_formula_weight         2607.19
_chemical_name_common            'barium copper indium nitride'
_chemical_name_systematic
;
tetradecabarium dicopper tetraindium heptanitride
;
_space_group_IT_number           10
_symmetry_cell_setting           monoclinic
_symmetry_space_group_name_Hall  '-P 2y'
_symmetry_space_group_name_H-M   'P 1 2/m 1'
_atom_sites_solution_hydrogens   geom
_atom_sites_solution_primary     direct
_atom_sites_solution_secondary   difmap
_cell_angle_alpha                90
_cell_angle_beta                 102.263(5)
_cell_angle_gamma                90
_cell_formula_units_Z            2
_cell_length_a                   9.3225(19)
_cell_length_b                   8.0089(17)
_cell_length_c                   21.651(5)
_cell_measurement_reflns_used    892
_cell_measurement_temperature    293(2)
_cell_measurement_theta_max      31.08
_cell_measurement_theta_min      0.96
_cell_volume                     1579.6(6)
_computing_cell_refinement       'SMART and SAINT'
_computing_data_collection       'SMART and SAINT (Bruker, 1999)'
_computing_data_reduction        'XPREP (Bruker, 1997)'
_computing_molecular_graphics    'ATOMS (Dowty, 1999)'
_computing_publication_material  SHELXL97
_computing_structure_refinement  'SHELXL97 (Sheldrick, 1997)'
_computing_structure_solution    'SIR97 (Altomare et al., 1999)'
_diffrn_ambient_temperature      293(2)
_diffrn_measured_fraction_theta_full 0.992
_diffrn_measured_fraction_theta_max 0.992
_diffrn_measurement_device_type  'Bruker SMART CCD area-detector'
_diffrn_measurement_method       'ω scans'
_diffrn_radiation_monochromator  graphite
_diffrn_radiation_source         'fine-focus sealed tube'
_diffrn_radiation_type           MoK\a
_diffrn_radiation_wavelength     0.71073
_diffrn_reflns_av_R_equivalents  0.098
_diffrn_reflns_av_sigmaI/netI    0.087
_diffrn_reflns_limit_h_max       10
_diffrn_reflns_limit_h_min       -13
_diffrn_reflns_limit_k_max       11
_diffrn_reflns_limit_k_min       -10
_diffrn_reflns_limit_l_max       31
_diffrn_reflns_limit_l_min       -31
_diffrn_reflns_number            15245
_diffrn_reflns_theta_full        31.08
_diffrn_reflns_theta_max         31.08
_diffrn_reflns_theta_min         0.96
_diffrn_standards_decay_%        none
_exptl_absorpt_coefficient_mu    21.285
_exptl_absorpt_correction_T_max  0.330
_exptl_absorpt_correction_T_min  0.051
_exptl_absorpt_correction_type   analytical
_exptl_absorpt_process_details   'face-indexed (Reference?)'
_exptl_crystal_colour            black
_exptl_crystal_density_diffrn    5.481
_exptl_crystal_density_meas      ?
_exptl_crystal_density_method    'not measured'
_exptl_crystal_description       plate
_exptl_crystal_F_000             2174
_exptl_crystal_size_max          0.25
_exptl_crystal_size_mid          0.12
_exptl_crystal_size_min          0.06
_refine_diff_density_max         3.67
_refine_diff_density_min         -4.01
_refine_ls_extinction_coef       0.00084(5)
_refine_ls_extinction_expression Fc^*^=kFc[1+0.001xFc²λ³/sin(2θ)]^-1/4^
_refine_ls_extinction_method     'SHELXL97 (Sheldrick, 1997)'
_refine_ls_goodness_of_fit_ref   0.949
_refine_ls_hydrogen_treatment    none
_refine_ls_matrix_type           full
_refine_ls_number_parameters     151
_refine_ls_number_reflns         5370
_refine_ls_number_restraints     0
_refine_ls_restrained_S_all      0.949
_refine_ls_R_factor_all          0.080
_refine_ls_R_factor_gt           0.045
_refine_ls_shift/su_max          0.001
_refine_ls_shift/su_mean         0.000
_refine_ls_structure_factor_coef Fsqd
_refine_ls_weighting_details
'calc w = 1/[σ²(Fo²)+(0.0403P)²] where P=(Fo²+2Fc²)/3'
_refine_ls_weighting_scheme      calc
_refine_ls_wR_factor_gt          0.102
_refine_ls_wR_factor_ref         0.112
_reflns_number_gt                3463
_reflns_number_total             5370
_reflns_threshold_expression     I>2σ(I)
_cod_data_source_file            iz1020.cif
_cod_data_source_block           I
_cod_depositor_comments
;
The following automatic conversions were performed:

'_exptl_crystal_density_meas' value 'not measured' was changed to '?'
- the value is perceived as not measured.

Automatic conversion script
Id: cif_fix_values 3008 2015-01-20 13:52:24Z robertas 
;
_cod_original_cell_volume        1579.7(6)
_cod_original_sg_symbol_H-M      'P 2/m'
_cod_database_code               2012637
_cod_database_fobs_code          2012637
loop_
_symmetry_equiv_pos_as_xyz
'x, y, z'
'-x, y, -z'
'-x, -y, -z'
'x, -y, z'
loop_
_atom_site_label
_atom_site_fract_x
_atom_site_fract_y
_atom_site_fract_z
_atom_site_U_iso_or_equiv
_atom_site_adp_type
_atom_site_calc_flag
_atom_site_refinement_flags
_atom_site_occupancy
_atom_site_disorder_assembly
_atom_site_disorder_group
_atom_site_type_symbol
Ba1 0.25594(7) 0.24125(7) 0.10195(3) 0.02270(14) Uani d . 1 . . Ba
Ba2 0.42305(7) 0.24578(7) 0.30170(3) 0.02326(15) Uani d . 1 . . Ba
Ba3 0.82694(6) 0.25274(7) 0.08070(3) 0.01840(13) Uani d . 1 . . Ba
Ba4 0.16404(9) 0.5000 0.40728(4) 0.01613(17) Uani d S 1 . . Ba
Ba5 0.24922(9) 0.5000 0.58451(4) 0.01539(17) Uani d S 1 . . Ba
Ba6 0.08425(9) 0.0000 0.21101(4) 0.01703(18) Uani d S 1 . . Ba
Ba7 0.16238(10) 0.0000 0.40723(4) 0.02093(19) Uani d S 1 . . Ba
Ba8 0.24943(10) 0.0000 0.58943(4) 0.02001(19) Uani d S 1 . . Ba
Ba9 0.60738(9) 0.0000 0.18409(5) 0.02102(19) Uani d S 1 . . Ba
Ba10 0.5000 0.23813(12) 0.5000 0.0398(3) Uani d S 1 . . Ba
Ba11 0.5000 0.5000 0.0000 0.0258(3) Uani d S 1 . . Ba
Ba12 0.5000 0.0000 0.0000 0.0324(3) Uani d S 1 . . Ba
In1 0.13605(9) 0.29393(9) 0.71845(4) 0.02444(18) Uani d . 1 . . In
In2 0.05646(12) 0.5000 0.21941(6) 0.0240(2) Uani d S 1 . . In
In3 0.64793(13) 0.5000 0.19432(6) 0.0281(3) Uani d S 1 . . In
Cu1 0.0000 0.24712(19) 0.5000 0.0151(3) Uani d S 1 . . Cu
Cu2 0.0000 0.5000 0.0000 0.0145(5) Uani d S 1 . . Cu
Cu3 0.0000 0.0000 0.0000 0.0162(5) Uani d S 1 . . Cu
N1 0.2005(8) 0.2450(9) 0.4959(4) 0.0182(16) Uani d . 1 . . N
N2 0.2070(12) 0.5000 0.0060(6) 0.018(2) Uani d S 1 . . N
N3 0.4530(14) 0.5000 0.3969(7) 0.031(3) Uani d S 1 . . N
N4 0.0327(13) 0.0000 0.0890(6) 0.020(2) Uani d S 1 . . N
N5 0.3598(13) 0.0000 0.2075(6) 0.022(3) Uani d S 1 . . N
N6 0.4475(17) 0.0000 0.3861(6) 0.034(3) Uani d S 1 . . N
loop_
_atom_type_symbol
_atom_type_description
_atom_type_scat_dispersion_real
_atom_type_scat_dispersion_imag
_atom_type_scat_source
N N 0.0061 0.0033 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Cu Cu 0.3201 1.2651 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
In In -0.7276 1.3100 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Ba Ba -0.3244 2.2819 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
loop_
_geom_angle_atom_site_label_1
_geom_angle_atom_site_label_2
_geom_angle_atom_site_label_3
_geom_angle_site_symmetry_1
_geom_angle_site_symmetry_3
_geom_angle
_geom_angle_publ_flag
N1 Cu1 N1 2_556 . 179.0(5) yes
N2 Cu2 N2 3_565 . 180.0 yes
N4 Cu3 N4 3 . 180.0 yes
N4 Ba1 N2 . . 114.8(3) ?
N4 Ba1 N5 . . 75.2(3) ?
N2 Ba1 N5 . . 169.9(3) ?
N4 Ba1 Cu3 . . 32.8(2) ?
N2 Ba1 Cu3 . . 87.70(19) ?
N5 Ba1 Cu3 . . 101.15(18) ?
N4 Ba1 Cu2 . . 87.3(2) ?
N2 Ba1 Cu2 . . 32.4(2) ?
N5 Ba1 Cu2 . . 156.5(2) ?
Cu3 Ba1 Cu2 . . 69.486(19) ?
N4 Ba1 Ba6 . . 44.5(2) ?
N2 Ba1 Ba6 . . 144.4(2) ?
N5 Ba1 Ba6 . . 44.2(2) ?
Cu3 Ba1 Ba6 . . 77.38(2) ?
Cu2 Ba1 Ba6 . . 112.31(2) ?
N4 Ba1 Ba1 . 4 46.56(16) ?
N2 Ba1 Ba1 . 4 135.59(17) ?
N5 Ba1 Ba1 . 4 49.79(16) ?
Cu3 Ba1 Ba1 . 4 56.197(12) ?
Cu2 Ba1 Ba1 . 4 125.683(12) ?
Ba6 Ba1 Ba1 . 4 58.243(13) ?
N4 Ba1 Ba3 . 2_655 86.1(2) ?
N2 Ba1 Ba3 . 2_655 44.24(17) ?
N5 Ba1 Ba3 . 2_655 139.34(17) ?
Cu3 Ba1 Ba3 . 2_655 53.276(14) ?
Cu2 Ba1 Ba3 . 2_655 52.314(14) ?
Ba6 Ba1 Ba3 . 2_655 130.60(2) ?
Ba1 Ba1 Ba3 4 2_655 91.364(12) ?
N4 Ba1 Ba9 . . 103.77(19) ?
N2 Ba1 Ba9 . . 132.1(2) ?
N5 Ba1 Ba9 . . 39.3(2) ?
Cu3 Ba1 Ba9 . . 114.34(2) ?
Cu2 Ba1 Ba9 . . 164.22(2) ?
Ba6 Ba1 Ba9 . . 83.37(2) ?
Ba1 Ba1 Ba9 4 . 60.244(13) ?
Ba3 Ba1 Ba9 2_655 . 116.43(2) ?
N4 Ba1 Ba3 . 1_455 44.79(16) ?
N2 Ba1 Ba3 . 1_455 84.2(2) ?
N5 Ba1 Ba3 . 1_455 105.1(2) ?
Cu3 Ba1 Ba3 . 1_455 52.679(15) ?
Cu2 Ba1 Ba3 . 1_455 51.753(14) ?
Ba6 Ba1 Ba3 . 1_455 61.02(2) ?
Ba1 Ba1 Ba3 4 1_455 91.343(12) ?
Ba3 Ba1 Ba3 2_655 1_455 84.398(19) ?
Ba9 Ba1 Ba3 . 1_455 143.34(2) ?
N4 Ba1 Ba12 . . 96.27(19) ?
N2 Ba1 Ba12 . . 88.35(18) ?
N5 Ba1 Ba12 . . 88.85(19) ?
Cu3 Ba1 Ba12 . . 76.966(19) ?
Cu2 Ba1 Ba12 . . 108.99(2) ?
Ba6 Ba1 Ba12 . . 118.61(2) ?
Ba1 Ba1 Ba12 4 . 61.033(10) ?
Ba3 Ba1 Ba12 2_655 . 57.257(15) ?
Ba9 Ba1 Ba12 . . 59.26(2) ?
Ba3 Ba1 Ba12 1_455 . 129.24(2) ?
N4 Ba1 In2 . . 89.15(19) ?
N2 Ba1 In2 . . 93.51(18) ?
N5 Ba1 In2 . . 88.15(18) ?
Cu3 Ba1 In2 . . 109.91(3) ?
Cu2 Ba1 In2 . . 75.70(2) ?
Ba6 Ba1 In2 . . 62.73(2) ?
Ba1 Ba1 In2 4 . 120.957(13) ?
Ba3 Ba1 In2 2_655 . 127.93(3) ?
Ba9 Ba1 In2 . . 115.05(3) ?
Ba3 Ba1 In2 1_455 . 57.79(2) ?
Ba12 Ba1 In2 . . 172.93(2) ?
N6 Ba2 N5 . . 87.4(3) ?
N6 Ba2 N3 . . 92.9(3) ?
N5 Ba2 N3 . . 173.6(3) ?
N6 Ba2 Ba6 . . 85.1(3) ?
N5 Ba2 Ba6 . . 41.7(2) ?
N3 Ba2 Ba6 . . 131.9(2) ?
N6 Ba2 Ba9 . . 95.1(2) ?
N5 Ba2 Ba9 . . 39.1(2) ?
N3 Ba2 Ba9 . . 147.1(2) ?
Ba6 Ba2 Ba9 . . 80.66(2) ?
N6 Ba2 Ba2 . 4 42.3(2) ?
N5 Ba2 Ba2 . 4 45.44(19) ?
N3 Ba2 Ba2 . 4 135.2(2) ?
Ba6 Ba2 Ba2 . 4 59.534(13) ?
Ba9 Ba2 Ba2 . 4 59.644(12) ?
N6 Ba2 Ba8 . 3_656 44.1(3) ?
N5 Ba2 Ba8 . 3_656 95.8(2) ?
N3 Ba2 Ba8 . 3_656 88.9(2) ?
Ba6 Ba2 Ba8 . 3_656 119.37(2) ?
Ba9 Ba2 Ba8 . 3_656 75.32(3) ?
Ba2 Ba2 Ba8 4 3_656 60.209(13) ?
N6 Ba2 In3 . . 142.7(3) ?
N5 Ba2 In3 . . 89.4(2) ?
N3 Ba2 In3 . . 94.2(2) ?
Ba6 Ba2 In3 . . 115.75(3) ?
Ba9 Ba2 In3 . . 61.251(19) ?
Ba2 Ba2 In3 4 . 120.581(13) ?
Ba8 Ba2 In3 3_656 . 99.54(3) ?
N6 Ba2 Ba5 . 3_666 90.6(3) ?
N5 Ba2 Ba5 . 3_666 144.2(2) ?
N3 Ba2 Ba5 . 3_666 42.2(3) ?
Ba6 Ba2 Ba5 . 3_666 172.60(3) ?
Ba9 Ba2 Ba5 . 3_666 105.76(3) ?
Ba2 Ba2 Ba5 4 3_666 120.232(12) ?
Ba8 Ba2 Ba5 3_656 3_666 60.039(19) ?
In3 Ba2 Ba5 . 3_666 71.13(3) ?
N6 Ba2 In2 . . 127.9(3) ?
N5 Ba2 In2 . . 90.3(2) ?
N3 Ba2 In2 . . 84.5(3) ?
Ba6 Ba2 In2 . . 60.84(2) ?
Ba9 Ba2 In2 . . 114.49(3) ?
Ba2 Ba2 In2 4 . 120.170(13) ?
Ba8 Ba2 In2 3_656 . 169.38(3) ?
In3 Ba2 In2 . . 89.19(3) ?
Ba5 Ba2 In2 3_666 . 118.20(2) ?
N6 Ba2 Ba2 . 4_565 137.7(2) ?
N5 Ba2 Ba2 . 4_565 134.56(19) ?
N3 Ba2 Ba2 . 4_565 44.8(2) ?
Ba6 Ba2 Ba2 . 4_565 120.467(13) ?
Ba9 Ba2 Ba2 . 4_565 120.356(12) ?
Ba2 Ba2 Ba2 4 4_565 180.00(6) ?
Ba8 Ba2 Ba2 3_656 4_565 119.791(13) ?
In3 Ba2 Ba2 . 4_565 59.419(13) ?
Ba5 Ba2 Ba2 3_666 4_565 59.768(12) ?
In2 Ba2 Ba2 . 4_565 59.830(13) ?
N6 Ba2 Ba7 . . 41.3(3) ?
N5 Ba2 Ba7 . . 90.6(2) ?
N3 Ba2 Ba7 . . 85.4(2) ?
Ba6 Ba2 Ba7 . . 62.04(2) ?
Ba9 Ba2 Ba7 . . 120.63(2) ?
Ba2 Ba2 Ba7 4 . 61.807(12) ?
Ba8 Ba2 Ba7 3_656 . 84.52(2) ?
In3 Ba2 Ba7 . . 175.91(3) ?
Ba5 Ba2 Ba7 3_666 . 110.91(3) ?
In2 Ba2 Ba7 . . 86.72(3) ?
Ba2 Ba2 Ba7 4_565 . 118.193(12) ?
N2 Ba3 N4 3_665 1_655 124.0(3) ?
N2 Ba3 Cu2 3_665 1_655 35.5(2) ?
N4 Ba3 Cu2 1_655 1_655 93.65(19) ?
N2 Ba3 Cu3 3_665 1_655 94.58(19) ?
N4 Ba3 Cu3 1_655 1_655 34.7(2) ?
Cu2 Ba3 Cu3 1_655 1_655 74.816(19) ?
N2 Ba3 Ba11 3_665 . 47.5(2) ?
N4 Ba3 Ba11 1_655 . 154.4(2) ?
Cu2 Ba3 Ba11 1_655 . 82.868(19) ?
Cu3 Ba3 Ba11 1_655 . 121.15(2) ?
N2 Ba3 Ba12 3_665 . 96.2(2) ?
N4 Ba3 Ba12 1_655 . 96.8(2) ?
Cu2 Ba3 Ba12 1_655 . 121.21(2) ?
Cu3 Ba3 Ba12 1_655 . 82.155(19) ?
Ba11 Ba3 Ba12 . . 64.471(17) ?
N2 Ba3 In3 3_665 . 93.73(19) ?
N4 Ba3 In3 1_655 . 137.0(2) ?
Cu2 Ba3 In3 1_655 . 111.25(2) ?
Cu3 Ba3 In3 1_655 . 171.44(2) ?
Ba11 Ba3 In3 . . 66.50(2) ?
Ba12 Ba3 In3 . . 99.02(2) ?
N2 Ba3 In2 3_665 1_655 97.4(2) ?
N4 Ba3 In2 1_655 1_655 93.6(2) ?
Cu2 Ba3 In2 1_655 1_655 81.39(2) ?
Cu3 Ba3 In2 1_655 1_655 118.33(3) ?
Ba11 Ba3 In2 . 1_655 110.80(2) ?
Ba12 Ba3 In2 . 1_655 154.22(2) ?
In3 Ba3 In2 . 1_655 58.35(3) ?
N2 Ba3 Ba6 3_665 1_655 148.7(2) ?
N4 Ba3 Ba6 1_655 1_655 41.9(2) ?
Cu2 Ba3 Ba6 1_655 1_655 113.93(2) ?
Cu3 Ba3 Ba6 1_655 1_655 76.61(2) ?
Ba11 Ba3 Ba6 . 1_655 159.35(2) ?
Ba12 Ba3 Ba6 . 1_655 111.90(2) ?
In3 Ba3 Ba6 . 1_655 95.16(3) ?
In2 Ba3 Ba6 1_655 1_655 62.84(2) ?
N2 Ba3 Ba1 3_665 2_655 48.55(19) ?
N4 Ba3 Ba1 1_655 2_655 92.0(2) ?
Cu2 Ba3 Ba1 1_655 2_655 58.928(16) ?
Cu3 Ba3 Ba1 1_655 2_655 57.264(15) ?
Ba11 Ba3 Ba1 . 2_655 64.465(15) ?
Ba12 Ba3 Ba1 . 2_655 63.019(15) ?
In3 Ba3 Ba1 . 2_655 130.80(3) ?
In2 Ba3 Ba1 1_655 2_655 140.20(2) ?
Ba6 Ba3 Ba1 1_655 2_655 133.83(2) ?
N2 Ba3 Ba9 3_665 . 141.3(2) ?
N4 Ba3 Ba9 1_655 . 91.38(19) ?
Cu2 Ba3 Ba9 1_655 . 174.121(19) ?
Cu3 Ba3 Ba9 1_655 . 111.06(2) ?
Ba11 Ba3 Ba9 . . 93.89(2) ?
Ba12 Ba3 Ba9 . . 61.06(2) ?
In3 Ba3 Ba9 . . 62.885(19) ?
In2 Ba3 Ba9 1_655 . 95.26(3) ?
Ba6 Ba3 Ba9 1_655 . 68.26(2) ?
Ba1 Ba3 Ba9 2_655 . 123.98(2) ?
N2 Ba3 Ba1 3_665 1_655 93.7(2) ?
N4 Ba3 Ba1 1_655 1_655 45.66(18) ?
Cu2 Ba3 Ba1 1_655 1_655 58.213(15) ?
Cu3 Ba3 Ba1 1_655 1_655 56.573(14) ?
Ba11 Ba3 Ba1 . 1_655 140.810(19) ?
Ba12 Ba3 Ba1 . 1_655 138.19(2) ?
In3 Ba3 Ba1 . 1_655 120.76(3) ?
In2 Ba3 Ba1 1_655 1_655 62.41(2) ?
Ba6 Ba3 Ba1 1_655 1_655 56.198(18) ?
Ba1 Ba3 Ba1 2_655 1_655 95.538(19) ?
Ba9 Ba3 Ba1 . 1_655 124.43(2) ?
N3 Ba4 N1 . 4_565 94.5(3) ?
N3 Ba4 N1 . . 94.5(3) ?
N1 Ba4 N1 4_565 . 94.9(3) ?
N3 Ba4 Cu1 . . 127.9(2) ?
N1 Ba4 Cu1 4_565 . 91.96(16) ?
N1 Ba4 Cu1 . . 33.39(15) ?
N3 Ba4 Cu1 . 3_566 127.9(2) ?
N1 Ba4 Cu1 4_565 3_566 33.39(15) ?
N1 Ba4 Cu1 . 3_566 91.96(16) ?
Cu1 Ba4 Cu1 . 3_566 72.34(5) ?
N3 Ba4 Ba5 . . 94.9(3) ?
N1 Ba4 Ba5 4_565 . 47.45(17) ?
N1 Ba4 Ba5 . . 47.45(17) ?
Cu1 Ba4 Ba5 . . 54.91(2) ?
Cu1 Ba4 Ba5 3_566 . 54.91(2) ?
N3 Ba4 In1 . 2_556 121.4(3) ?
N1 Ba4 In1 4_565 2_556 140.48(16) ?
N1 Ba4 In1 . 2_556 97.93(17) ?
Cu1 Ba4 In1 . 2_556 79.21(2) ?
Cu1 Ba4 In1 3_566 2_556 108.69(3) ?
Ba5 Ba4 In1 . 2_556 133.63(2) ?
N3 Ba4 In1 . 3_566 121.4(3) ?
N1 Ba4 In1 4_565 3_566 97.93(17) ?
N1 Ba4 In1 . 3_566 140.48(16) ?
Cu1 Ba4 In1 . 3_566 108.69(3) ?
Cu1 Ba4 In1 3_566 3_566 79.21(2) ?
Ba5 Ba4 In1 . 3_566 133.63(2) ?
In1 Ba4 In1 2_556 3_566 50.95(3) ?
N3 Ba4 Ba5 . 3_566 178.0(3) ?
N1 Ba4 Ba5 4_565 3_566 86.88(15) ?
N1 Ba4 Ba5 . 3_566 86.88(15) ?
Cu1 Ba4 Ba5 . 3_566 53.498(18) ?
Cu1 Ba4 Ba5 3_566 3_566 53.498(18) ?
Ba5 Ba4 Ba5 . 3_566 87.12(3) ?
In1 Ba4 Ba5 2_556 3_566 56.85(2) ?
In1 Ba4 Ba5 3_566 3_566 56.85(2) ?
N3 Ba4 Ba10 . 3_666 49.9(2) ?
N1 Ba4 Ba10 4_565 3_666 44.69(15) ?
N1 Ba4 Ba10 . 3_666 94.12(17) ?
Cu1 Ba4 Ba10 . 3_666 114.85(3) ?
Cu1 Ba4 Ba10 3_566 3_666 78.04(2) ?
Ba5 Ba4 Ba10 . 3_666 60.437(17) ?
In1 Ba4 Ba10 2_556 3_666 165.90(3) ?
In1 Ba4 Ba10 3_566 3_666 120.84(2) ?
Ba5 Ba4 Ba10 3_566 3_666 131.52(2) ?
N3 Ba4 Ba10 . . 49.9(2) ?
N1 Ba4 Ba10 4_565 . 94.12(17) ?
N1 Ba4 Ba10 . . 44.69(15) ?
Cu1 Ba4 Ba10 . . 78.04(2) ?
Cu1 Ba4 Ba10 3_566 . 114.85(3) ?
Ba5 Ba4 Ba10 . . 60.437(17) ?
In1 Ba4 Ba10 2_556 . 120.84(2) ?
In1 Ba4 Ba10 3_566 . 165.90(3) ?
Ba5 Ba4 Ba10 3_566 . 131.52(2) ?
Ba10 Ba4 Ba10 3_666 . 64.22(3) ?
N3 Ba4 In2 . . 87.4(3) ?
N1 Ba4 In2 4_565 . 132.44(17) ?
N1 Ba4 In2 . . 132.44(17) ?
Cu1 Ba4 In2 . . 123.47(2) ?
Cu1 Ba4 In2 3_566 . 123.47(2) ?
Ba5 Ba4 In2 . . 177.68(3) ?
In1 Ba4 In2 2_556 . 44.52(2) ?
In1 Ba4 In2 3_566 . 44.52(2) ?
Ba5 Ba4 In2 3_566 . 90.55(3) ?
Ba10 Ba4 In2 3_666 . 121.39(2) ?
Ba10 Ba4 In2 . . 121.39(2) ?
N3 Ba5 N1 3_666 . 96.6(3) ?
N3 Ba5 N1 3_666 4_565 96.6(3) ?
N1 Ba5 N1 . 4_565 94.9(3) ?
N3 Ba5 Cu1 3_666 . 130.83(18) ?
N1 Ba5 Cu1 . . 34.67(15) ?
N1 Ba5 Cu1 4_565 . 94.31(17) ?
N3 Ba5 Cu1 3_666 3_566 130.83(18) ?
N1 Ba5 Cu1 . 3_566 94.31(17) ?
N1 Ba5 Cu1 4_565 3_566 34.67(15) ?
Cu1 Ba5 Cu1 . 3_566 75.10(5) ?
N3 Ba5 In1 3_666 4_565 109.8(3) ?
N1 Ba5 In1 . 4_565 147.50(16) ?
N1 Ba5 In1 4_565 4_565 100.54(16) ?
Cu1 Ba5 In1 . 4_565 115.04(3) ?
Cu1 Ba5 In1 3_566 4_565 82.92(2) ?
N3 Ba5 In1 3_666 . 109.8(3) ?
N1 Ba5 In1 . . 100.54(16) ?
N1 Ba5 In1 4_565 . 147.50(15) ?
Cu1 Ba5 In1 . . 82.92(2) ?
Cu1 Ba5 In1 3_566 . 115.04(3) ?
In1 Ba5 In1 4_565 . 53.29(3) ?
N3 Ba5 Ba4 3_666 . 98.0(3) ?
N1 Ba5 Ba4 . . 47.45(16) ?
N1 Ba5 Ba4 4_565 . 47.45(16) ?
Cu1 Ba5 Ba4 . . 57.67(2) ?
Cu1 Ba5 Ba4 3_566 . 57.67(2) ?
In1 Ba5 Ba4 4_565 . 140.57(3) ?
In1 Ba5 Ba4 . . 140.57(3) ?
N3 Ba5 Ba10 3_666 3_666 51.0(2) ?
N1 Ba5 Ba10 . 3_666 95.64(16) ?
N1 Ba5 Ba10 4_565 3_666 45.69(15) ?
Cu1 Ba5 Ba10 . 3_666 119.41(3) ?
Cu1 Ba5 Ba10 3_566 3_666 80.30(2) ?
In1 Ba5 Ba10 4_565 3_666 115.58(2) ?
In1 Ba5 Ba10 . 3_666 156.49(3) ?
Ba4 Ba5 Ba10 . 3_666 62.281(18) ?
N3 Ba5 Ba10 3_666 . 51.0(2) ?
N1 Ba5 Ba10 . . 45.69(15) ?
N1 Ba5 Ba10 4_565 . 95.64(16) ?
Cu1 Ba5 Ba10 . . 80.30(2) ?
Cu1 Ba5 Ba10 3_566 . 119.41(3) ?
In1 Ba5 Ba10 4_565 . 156.49(3) ?
In1 Ba5 Ba10 . . 115.58(2) ?
Ba4 Ba5 Ba10 . . 62.281(18) ?
Ba10 Ba5 Ba10 3_666 . 65.50(3) ?
N3 Ba5 Ba4 3_666 3_566 169.1(3) ?
N1 Ba5 Ba4 . 3_566 90.77(15) ?
N1 Ba5 Ba4 4_565 3_566 90.77(15) ?
Cu1 Ba5 Ba4 . 3_566 56.11(2) ?
Cu1 Ba5 Ba4 3_566 3_566 56.11(2) ?
In1 Ba5 Ba4 4_565 3_566 60.80(2) ?
In1 Ba5 Ba4 . 3_566 60.80(2) ?
Ba4 Ba5 Ba4 . 3_566 92.88(3) ?
Ba10 Ba5 Ba4 3_666 3_566 136.32(2) ?
Ba10 Ba5 Ba4 . 3_566 136.32(2) ?
N3 Ba5 Ba8 3_666 1_565 90.08(2) ?
N1 Ba5 Ba8 . 1_565 138.91(17) ?
N1 Ba5 Ba8 4_565 1_565 44.05(16) ?
Cu1 Ba5 Ba8 . 1_565 128.33(4) ?
Cu1 Ba5 Ba8 3_566 1_565 53.25(3) ?
In1 Ba5 Ba8 4_565 1_565 61.926(19) ?
In1 Ba5 Ba8 . 1_565 115.21(3) ?
Ba4 Ba5 Ba8 . 1_565 91.490(19) ?
Ba10 Ba5 Ba8 3_666 1_565 58.320(19) ?
Ba10 Ba5 Ba8 . 1_565 123.81(3) ?
Ba4 Ba5 Ba8 3_566 1_565 89.638(17) ?
N4 Ba6 N5 . . 86.6(4) ?
N4 Ba6 In1 . 3_556 115.30(18) ?
N5 Ba6 In1 . 3_556 131.33(15) ?
N4 Ba6 In1 . 2_556 115.30(18) ?
N5 Ba6 In1 . 2_556 131.33(15) ?
In1 Ba6 In1 3_556 2_556 79.95(3) ?
N4 Ba6 Ba1 . 4 49.76(19) ?
N5 Ba6 Ba1 . 4 53.8(2) ?
In1 Ba6 Ba1 3_556 4 106.83(2) ?
In1 Ba6 Ba1 2_556 4 164.99(3) ?
N4 Ba6 Ba1 . . 49.76(19) ?
N5 Ba6 Ba1 . . 53.8(2) ?
In1 Ba6 Ba1 3_556 . 164.99(3) ?
In1 Ba6 Ba1 2_556 . 106.83(2) ?
Ba1 Ba6 Ba1 4 . 63.51(3) ?
N4 Ba6 Ba3 . 4_455 45.69(18) ?
N5 Ba6 Ba3 . 4_455 116.4(2) ?
In1 Ba6 Ba3 3_556 4_455 69.63(2) ?
In1 Ba6 Ba3 2_556 4_455 108.96(3) ?
Ba1 Ba6 Ba3 4 4_455 62.78(2) ?
Ba1 Ba6 Ba3 . 4_455 95.39(3) ?
N4 Ba6 Ba3 . 1_455 45.69(17) ?
N5 Ba6 Ba3 . 1_455 116.4(2) ?
In1 Ba6 Ba3 3_556 1_455 108.96(3) ?
In1 Ba6 Ba3 2_556 1_455 69.63(2) ?
Ba1 Ba6 Ba3 4 1_455 95.39(3) ?
Ba1 Ba6 Ba3 . 1_455 62.78(2) ?
Ba3 Ba6 Ba3 4_455 1_455 63.17(3) ?
N4 Ba6 Ba2 . . 118.2(2) ?
N5 Ba6 Ba2 . . 46.2(2) ?
In1 Ba6 Ba2 3_556 . 125.65(3) ?
In1 Ba6 Ba2 2_556 . 86.06(2) ?
Ba1 Ba6 Ba2 4 . 99.97(3) ?
Ba1 Ba6 Ba2 . . 68.86(2) ?
Ba3 Ba6 Ba2 4_455 . 161.25(3) ?
Ba3 Ba6 Ba2 1_455 . 114.570(19) ?
N4 Ba6 Ba2 . 4 118.2(2) ?
N5 Ba6 Ba2 . 4 46.2(2) ?
In1 Ba6 Ba2 3_556 4 86.06(2) ?
In1 Ba6 Ba2 2_556 4 125.65(3) ?
Ba1 Ba6 Ba2 4 4 68.86(2) ?
Ba1 Ba6 Ba2 . 4 99.97(3) ?
Ba3 Ba6 Ba2 4_455 4 114.570(19) ?
Ba3 Ba6 Ba2 1_455 4 161.25(3) ?
Ba2 Ba6 Ba2 . 4 60.93(3) ?
N4 Ba6 In2 . 1_545 92.67(3) ?
N5 Ba6 In2 . 1_545 94.32(2) ?
In1 Ba6 In2 3_556 1_545 45.075(19) ?
In1 Ba6 In2 2_556 1_545 125.03(3) ?
Ba1 Ba6 In2 4 1_545 62.99(2) ?
Ba1 Ba6 In2 . 1_545 126.48(3) ?
Ba3 Ba6 In2 4_455 1_545 58.35(2) ?
Ba3 Ba6 In2 1_455 1_545 121.26(3) ?
Ba2 Ba6 In2 . 1_545 122.38(3) ?
Ba2 Ba6 In2 4 1_545 61.66(2) ?
N4 Ba6 In2 . . 92.67(3) ?
N5 Ba6 In2 . . 94.32(2) ?
In1 Ba6 In2 3_556 . 125.03(3) ?
In1 Ba6 In2 2_556 . 45.075(19) ?
Ba1 Ba6 In2 4 . 126.48(3) ?
Ba1 Ba6 In2 . . 62.99(2) ?
Ba3 Ba6 In2 4_455 . 121.26(3) ?
Ba3 Ba6 In2 1_455 . 58.35(2) ?
Ba2 Ba6 In2 . . 61.66(2) ?
Ba2 Ba6 In2 4 . 122.38(3) ?
In2 Ba6 In2 1_545 . 170.10(4) ?
N1 Ba7 N1 . 4 92.6(3) ?
N1 Ba7 N6 . . 97.5(2) ?
N1 Ba7 N6 4 . 97.5(2) ?
N1 Ba7 Cu1 . 3_556 90.63(16) ?
N1 Ba7 Cu1 4 3_556 33.76(16) ?
N6 Ba7 Cu1 . 3_556 131.04(18) ?
N1 Ba7 Cu1 . . 33.76(16) ?
N1 Ba7 Cu1 4 . 90.63(16) ?
N6 Ba7 Cu1 . . 131.04(18) ?
Cu1 Ba7 Cu1 3_556 . 71.29(5) ?
N1 Ba7 Ba8 . . 46.30(17) ?
N1 Ba7 Ba8 4 . 46.30(17) ?
N6 Ba7 Ba8 . . 99.6(3) ?
Cu1 Ba7 Ba8 3_556 . 54.42(2) ?
Cu1 Ba7 Ba8 . . 54.42(2) ?
N1 Ba7 Ba8 . 3_556 88.17(16) ?
N1 Ba7 Ba8 4 3_556 88.17(16) ?
N6 Ba7 Ba8 . 3_556 171.8(3) ?
Cu1 Ba7 Ba8 3_556 3_556 54.420(19) ?
Cu1 Ba7 Ba8 . 3_556 54.42(2) ?
Ba8 Ba7 Ba8 . 3_556 88.56(3) ?
N1 Ba7 Ba10 . . 45.97(16) ?
N1 Ba7 Ba10 4 . 91.11(17) ?
N6 Ba7 Ba10 . . 52.1(2) ?
Cu1 Ba7 Ba10 3_556 . 113.38(3) ?
Cu1 Ba7 Ba10 . . 79.68(2) ?
Ba8 Ba7 Ba10 . . 59.750(19) ?
Ba8 Ba7 Ba10 3_556 . 134.07(2) ?
N1 Ba7 Ba10 . 3_656 91.11(17) ?
N1 Ba7 Ba10 4 3_656 45.97(16) ?
N6 Ba7 Ba10 . 3_656 52.1(2) ?
Cu1 Ba7 Ba10 3_556 3_656 79.68(2) ?
Cu1 Ba7 Ba10 . 3_656 113.38(3) ?
Ba8 Ba7 Ba10 . 3_656 59.750(19) ?
Ba8 Ba7 Ba10 3_556 3_656 134.07(2) ?
Ba10 Ba7 Ba10 . 3_656 59.23(3) ?
N1 Ba7 Ba4 . . 43.71(17) ?
N1 Ba7 Ba4 4 . 136.27(17) ?
N6 Ba7 Ba4 . . 89.788(17) ?
Cu1 Ba7 Ba4 3_556 . 125.79(3) ?
Cu1 Ba7 Ba4 . . 54.50(3) ?
Ba8 Ba7 Ba4 . . 89.986(19) ?
Ba8 Ba7 Ba4 3_556 . 90.217(17) ?
Ba10 Ba7 Ba4 . . 60.20(2) ?
Ba10 Ba7 Ba4 3_656 . 119.43(3) ?
N1 Ba7 Ba4 . 1_545 136.27(17) ?
N1 Ba7 Ba4 4 1_545 43.71(17) ?
N6 Ba7 Ba4 . 1_545 89.788(17) ?
Cu1 Ba7 Ba4 3_556 1_545 54.50(3) ?
Cu1 Ba7 Ba4 . 1_545 125.79(3) ?
Ba8 Ba7 Ba4 . 1_545 89.986(19) ?
Ba8 Ba7 Ba4 3_556 1_545 90.217(18) ?
Ba10 Ba7 Ba4 . 1_545 119.43(3) ?
Ba10 Ba7 Ba4 3_656 1_545 60.20(2) ?
Ba4 Ba7 Ba4 . 1_545 179.56(4) ?
N1 Ba7 Ba6 . . 133.71(17) ?
N1 Ba7 Ba6 4 . 133.71(17) ?
N6 Ba7 Ba6 . . 78.4(3) ?
Cu1 Ba7 Ba6 3_556 . 126.97(3) ?
Cu1 Ba7 Ba6 . . 126.97(3) ?
Ba8 Ba7 Ba6 . . 177.99(3) ?
Ba8 Ba7 Ba6 3_556 . 93.45(3) ?
Ba10 Ba7 Ba6 . . 118.60(2) ?
Ba10 Ba7 Ba6 3_656 . 118.60(2) ?
Ba4 Ba7 Ba6 . . 90.006(18) ?
Ba4 Ba7 Ba6 1_545 . 90.006(18) ?
N6 Ba8 N1 3_656 4 98.2(2) ?
N6 Ba8 N1 3_656 . 98.2(2) ?
N1 Ba8 N1 4 . 89.5(3) ?
N6 Ba8 Cu1 3_656 3_556 131.99(17) ?
N1 Ba8 Cu1 4 3_556 34.46(15) ?
N1 Ba8 Cu1 . 3_556 90.56(17) ?
N6 Ba8 Cu1 3_656 . 131.99(17) ?
N1 Ba8 Cu1 4 . 90.56(17) ?
N1 Ba8 Cu1 . . 34.46(15) ?
Cu1 Ba8 Cu1 3_556 . 72.66(5) ?
N6 Ba8 Ba10 3_656 . 52.4(2) ?
N1 Ba8 Ba10 4 . 90.37(16) ?
N1 Ba8 Ba10 . . 46.17(15) ?
Cu1 Ba8 Ba10 3_556 . 115.14(3) ?
Cu1 Ba8 Ba10 . . 80.60(2) ?
N6 Ba8 Ba10 3_656 3_656 52.4(2) ?
N1 Ba8 Ba10 4 3_656 46.17(15) ?
N1 Ba8 Ba10 . 3_656 90.37(16) ?
Cu1 Ba8 Ba10 3_556 3_656 80.60(2) ?
Cu1 Ba8 Ba10 . 3_656 115.14(3) ?
Ba10 Ba8 Ba10 . 3_656 59.52(3) ?
N6 Ba8 Ba7 3_656 . 100.4(3) ?
N1 Ba8 Ba7 4 . 44.77(17) ?
N1 Ba8 Ba7 . . 44.77(17) ?
Cu1 Ba8 Ba7 3_556 . 55.78(2) ?
Cu1 Ba8 Ba7 . . 55.78(2) ?
Ba10 Ba8 Ba7 . . 60.18(2) ?
Ba10 Ba8 Ba7 3_656 . 60.178(19) ?
N6 Ba8 Ba7 3_656 3_556 168.1(3) ?
N1 Ba8 Ba7 4 3_556 90.22(15) ?
N1 Ba8 Ba7 . 3_556 90.22(15) ?
Cu1 Ba8 Ba7 3_556 3_556 55.78(2) ?
Cu1 Ba8 Ba7 . 3_556 55.78(2) ?
Ba10 Ba8 Ba7 . 3_556 136.38(2) ?
Ba10 Ba8 Ba7 3_656 3_556 136.38(2) ?
Ba7 Ba8 Ba7 . 3_556 91.44(3) ?
N6 Ba8 Ba2 3_656 2_656 42.10(18) ?
N1 Ba8 Ba2 4 2_656 140.22(16) ?
N1 Ba8 Ba2 . 2_656 93.95(17) ?
Cu1 Ba8 Ba2 3_556 2_656 173.11(3) ?
Cu1 Ba8 Ba2 . 2_656 113.83(3) ?
Ba10 Ba8 Ba2 . 2_656 65.10(2) ?
Ba10 Ba8 Ba2 3_656 2_656 94.14(3) ?
Ba7 Ba8 Ba2 . 2_656 125.24(2) ?
Ba7 Ba8 Ba2 3_556 2_656 129.31(3) ?
N6 Ba8 Ba2 3_656 3_656 42.10(18) ?
N1 Ba8 Ba2 4 3_656 93.95(16) ?
N1 Ba8 Ba2 . 3_656 140.22(16) ?
Cu1 Ba8 Ba2 3_556 3_656 113.83(3) ?
Cu1 Ba8 Ba2 . 3_656 173.11(3) ?
Ba10 Ba8 Ba2 . 3_656 94.14(3) ?
Ba10 Ba8 Ba2 3_656 3_656 65.10(2) ?
Ba7 Ba8 Ba2 . 3_656 125.24(2) ?
Ba7 Ba8 Ba2 3_556 3_656 129.31(3) ?
Ba2 Ba8 Ba2 2_656 3_656 59.58(3) ?
N6 Ba8 In1 3_656 . 106.2(2) ?
N1 Ba8 In1 4 . 154.58(15) ?
N1 Ba8 In1 . . 93.84(16) ?
Cu1 Ba8 In1 3_556 . 120.22(3) ?
Cu1 Ba8 In1 . . 78.45(2) ?
Ba10 Ba8 In1 . . 110.00(2) ?
Ba10 Ba8 In1 3_656 . 158.66(3) ?
Ba7 Ba8 In1 . . 133.74(2) ?
Ba7 Ba8 In1 3_556 . 64.61(2) ?
Ba2 Ba8 In1 2_656 . 64.71(2) ?
Ba2 Ba8 In1 3_656 . 99.38(3) ?
N5 Ba9 In1 . 2_656 113.8(2) ?
N5 Ba9 In1 . 3_656 113.8(2) ?
In1 Ba9 In1 2_656 3_656 79.43(3) ?
N5 Ba9 Ba1 . 4 50.2(2) ?
In1 Ba9 Ba1 2_656 4 163.71(3) ?
In1 Ba9 Ba1 3_656 4 109.00(2) ?
N5 Ba9 Ba1 . . 50.2(2) ?
In1 Ba9 Ba1 2_656 . 109.00(2) ?
In1 Ba9 Ba1 3_656 . 163.71(3) ?
Ba1 Ba9 Ba1 4 . 59.51(3) ?
N5 Ba9 Ba2 . . 45.8(2) ?
In1 Ba9 Ba2 2_656 . 68.01(2) ?
In1 Ba9 Ba2 3_656 . 105.75(3) ?
Ba1 Ba9 Ba2 4 . 95.98(3) ?
Ba1 Ba9 Ba2 . . 66.58(2) ?
N5 Ba9 Ba2 . 4 45.8(2) ?
In1 Ba9 Ba2 2_656 4 105.75(3) ?
In1 Ba9 Ba2 3_656 4 68.01(2) ?
Ba1 Ba9 Ba2 4 4 66.58(2) ?
Ba1 Ba9 Ba2 . 4 95.98(3) ?
Ba2 Ba9 Ba2 . 4 60.71(2) ?
N5 Ba9 Ba12 . . 99.3(3) ?
In1 Ba9 Ba12 2_656 . 125.47(2) ?
In1 Ba9 Ba12 3_656 . 125.47(2) ?
Ba1 Ba9 Ba12 4 . 61.604(18) ?
Ba1 Ba9 Ba12 . . 61.604(18) ?
Ba2 Ba9 Ba12 . . 127.98(2) ?
Ba2 Ba9 Ba12 4 . 127.98(2) ?
N5 Ba9 Ba3 . 4 138.20(19) ?
In1 Ba9 Ba3 2_656 4 107.70(3) ?
In1 Ba9 Ba3 3_656 4 68.99(2) ?
Ba1 Ba9 Ba3 4 4 88.49(2) ?
Ba1 Ba9 Ba3 . 4 119.23(3) ?
Ba2 Ba9 Ba3 . 4 174.07(3) ?
Ba2 Ba9 Ba3 4 4 118.075(18) ?
Ba12 Ba9 Ba3 . 4 57.712(18) ?
N5 Ba9 Ba3 . . 138.20(19) ?
In1 Ba9 Ba3 2_656 . 68.99(2) ?
In1 Ba9 Ba3 3_656 . 107.70(3) ?
Ba1 Ba9 Ba3 4 . 119.23(3) ?
Ba1 Ba9 Ba3 . . 88.49(2) ?
Ba2 Ba9 Ba3 . . 118.075(18) ?
Ba2 Ba9 Ba3 4 . 174.07(3) ?
Ba12 Ba9 Ba3 . . 57.712(18) ?
Ba3 Ba9 Ba3 4 . 62.46(2) ?
N5 Ba9 In3 . . 94.00(3) ?
In1 Ba9 In3 2_656 . 44.81(2) ?
In1 Ba9 In3 3_656 . 124.22(3) ?
Ba1 Ba9 In3 4 . 125.39(3) ?
Ba1 Ba9 In3 . . 65.88(2) ?
Ba2 Ba9 In3 . . 60.69(2) ?
Ba2 Ba9 In3 4 . 121.08(3) ?
Ba12 Ba9 In3 . . 93.27(2) ?
Ba3 Ba9 In3 4 . 119.54(3) ?
Ba3 Ba9 In3 . . 57.390(19) ?
N5 Ba9 In3 . 1_545 94.00(3) ?
In1 Ba9 In3 2_656 1_545 124.22(3) ?
In1 Ba9 In3 3_656 1_545 44.81(2) ?
Ba1 Ba9 In3 4 1_545 65.88(2) ?
Ba1 Ba9 In3 . 1_545 125.39(3) ?
Ba2 Ba9 In3 . 1_545 121.08(3) ?
Ba2 Ba9 In3 4 1_545 60.69(2) ?
Ba12 Ba9 In3 . 1_545 93.27(2) ?
Ba3 Ba9 In3 4 1_545 57.390(19) ?
Ba3 Ba9 In3 . 1_545 119.54(3) ?
In3 Ba9 In3 . 1_545 168.72(4) ?
N1 Ba10 N1 2_656 . 177.7(3) ?
N1 Ba10 N3 2_656 3_666 88.6(3) ?
N1 Ba10 N3 . 3_666 89.8(3) ?
N1 Ba10 N3 2_656 . 89.8(3) ?
N1 Ba10 N3 . . 88.6(3) ?
N3 Ba10 N3 3_666 . 92.2(4) ?
N1 Ba10 N6 2_656 . 91.5(3) ?
N1 Ba10 N6 . . 89.9(3) ?
N3 Ba10 N6 3_666 . 174.5(2) ?
N3 Ba10 N6 . . 82.2(3) ?
N1 Ba10 N6 2_656 3_656 89.9(3) ?
N1 Ba10 N6 . 3_656 91.5(3) ?
N3 Ba10 N6 3_666 3_656 82.2(3) ?
N3 Ba10 N6 . 3_656 174.5(2) ?
N6 Ba10 N6 . 3_656 103.3(3) ?
N1 Ba10 Ba10 2_656 3_656 91.14(16) ?
N1 Ba10 Ba10 . 3_656 91.14(16) ?
N3 Ba10 Ba10 3_666 3_656 133.88(19) ?
N3 Ba10 Ba10 . 3_656 133.88(19) ?
N6 Ba10 Ba10 . 3_656 51.65(16) ?
N6 Ba10 Ba10 3_656 3_656 51.65(16) ?
N1 Ba10 Ba8 2_656 . 135.15(17) ?
N1 Ba10 Ba8 . . 46.44(16) ?
N3 Ba10 Ba8 3_666 . 88.9(2) ?
N3 Ba10 Ba8 . . 135.0(2) ?
N6 Ba10 Ba8 . . 94.9(2) ?
N6 Ba10 Ba8 3_656 . 45.4(3) ?
Ba10 Ba10 Ba8 3_656 . 60.242(15) ?
N1 Ba10 Ba8 2_656 3_656 46.44(16) ?
N1 Ba10 Ba8 . 3_656 135.15(17) ?
N3 Ba10 Ba8 3_666 3_656 135.0(2) ?
N3 Ba10 Ba8 . 3_656 88.9(2) ?
N6 Ba10 Ba8 . 3_656 45.4(3) ?
N6 Ba10 Ba8 3_656 3_656 94.9(2) ?
Ba10 Ba10 Ba8 3_656 3_656 60.242(15) ?
Ba8 Ba10 Ba8 . 3_656 120.48(3) ?
N1 Ba10 Ba7 2_656 . 136.92(16) ?
N1 Ba10 Ba7 . . 44.71(17) ?
N3 Ba10 Ba7 3_666 . 134.5(2) ?
N3 Ba10 Ba7 . . 89.1(2) ?
N6 Ba10 Ba7 . . 45.8(3) ?
N6 Ba10 Ba7 3_656 . 94.8(2) ?
Ba10 Ba10 Ba7 3_656 . 60.383(16) ?
Ba8 Ba10 Ba7 . . 60.07(2) ?
Ba8 Ba10 Ba7 3_656 . 90.48(3) ?
N1 Ba10 Ba7 2_656 3_656 44.71(17) ?
N1 Ba10 Ba7 . 3_656 136.92(16) ?
N3 Ba10 Ba7 3_666 3_656 89.1(2) ?
N3 Ba10 Ba7 . 3_656 134.5(2) ?
N6 Ba10 Ba7 . 3_656 94.8(2) ?
N6 Ba10 Ba7 3_656 3_656 45.8(3) ?
Ba10 Ba10 Ba7 3_656 3_656 60.383(16) ?
Ba8 Ba10 Ba7 . 3_656 90.48(3) ?
Ba8 Ba10 Ba7 3_656 3_656 60.07(2) ?
Ba7 Ba10 Ba7 . 3_656 120.77(3) ?
N1 Ba10 Ba5 2_656 . 132.65(16) ?
N1 Ba10 Ba5 . . 45.64(17) ?
N3 Ba10 Ba5 3_666 . 44.3(2) ?
N3 Ba10 Ba5 . . 88.0(2) ?
N6 Ba10 Ba5 . . 134.9(3) ?
N6 Ba10 Ba5 3_656 . 88.1(2) ?
Ba10 Ba10 Ba5 3_656 . 122.750(15) ?
Ba8 Ba10 Ba5 . . 62.520(16) ?
Ba8 Ba10 Ba5 3_656 . 176.81(2) ?
Ba7 Ba10 Ba5 . . 90.35(2) ?
Ba7 Ba10 Ba5 3_656 . 121.91(2) ?
N2 Ba11 N2 . 3_665 180.0 ?
N2 Ba11 Ba3 . 2_655 46.08(17) ?
N2 Ba11 Ba3 3_665 2_655 133.92(17) ?
N2 Ba11 Ba3 . 4_565 133.92(17) ?
N2 Ba11 Ba3 3_665 4_565 46.08(17) ?
Ba3 Ba11 Ba3 2_655 4_565 180.0 ?
N2 Ba11 Ba3 . . 133.92(17) ?
N2 Ba11 Ba3 3_665 . 46.08(17) ?
Ba3 Ba11 Ba3 2_655 . 116.10(2) ?
Ba3 Ba11 Ba3 4_565 . 63.90(2) ?
N2 Ba11 Ba3 . 3_665 46.08(17) ?
N2 Ba11 Ba3 3_665 3_665 133.92(17) ?
Ba3 Ba11 Ba3 2_655 3_665 63.90(2) ?
Ba3 Ba11 Ba3 4_565 3_665 116.10(2) ?
Ba3 Ba11 Ba3 . 3_665 180.0 ?
N2 Ba11 Ba12 . 1_565 90.0 ?
N2 Ba11 Ba12 3_665 1_565 90.0 ?
Ba3 Ba11 Ba12 2_655 1_565 121.952(11) ?
Ba3 Ba11 Ba12 4_565 1_565 58.048(11) ?
Ba3 Ba11 Ba12 . 1_565 121.952(11) ?
Ba3 Ba11 Ba12 3_665 1_565 58.048(11) ?
N2 Ba11 Ba12 . . 90.0 ?
N2 Ba11 Ba12 3_665 . 90.0 ?
Ba3 Ba11 Ba12 2_655 . 58.048(11) ?
Ba3 Ba11 Ba12 4_565 . 121.952(11) ?
Ba3 Ba11 Ba12 . . 58.048(11) ?
Ba3 Ba11 Ba12 3_665 . 121.952(11) ?
Ba12 Ba11 Ba12 1_565 . 180.0 ?
N2 Ba11 Ba1 . 2_655 134.40(18) ?
N2 Ba11 Ba1 3_665 2_655 45.60(18) ?
Ba3 Ba11 Ba1 2_655 2_655 88.335(19) ?
Ba3 Ba11 Ba1 4_565 2_655 91.665(19) ?
Ba3 Ba11 Ba1 . 2_655 59.250(18) ?
Ba3 Ba11 Ba1 3_665 2_655 120.750(18) ?
Ba12 Ba11 Ba1 1_565 2_655 120.699(11) ?
Ba12 Ba11 Ba1 . 2_655 59.301(11) ?
N2 Ba11 Ba1 . 3_665 134.40(18) ?
N2 Ba11 Ba1 3_665 3_665 45.60(18) ?
Ba3 Ba11 Ba1 2_655 3_665 120.750(18) ?
Ba3 Ba11 Ba1 4_565 3_665 59.250(18) ?
Ba3 Ba11 Ba1 . 3_665 91.665(19) ?
Ba3 Ba11 Ba1 3_665 3_665 88.335(19) ?
Ba12 Ba11 Ba1 1_565 3_665 59.301(11) ?
Ba12 Ba11 Ba1 . 3_665 120.699(11) ?
Ba1 Ba11 Ba1 2_655 3_665 61.40(2) ?
N2 Ba11 Ba1 . . 45.60(18) ?
N2 Ba11 Ba1 3_665 . 134.40(18) ?
Ba3 Ba11 Ba1 2_655 . 59.250(18) ?
Ba3 Ba11 Ba1 4_565 . 120.750(18) ?
Ba3 Ba11 Ba1 . . 88.335(19) ?
Ba3 Ba11 Ba1 3_665 . 91.665(19) ?
Ba12 Ba11 Ba1 1_565 . 120.699(11) ?
Ba12 Ba11 Ba1 . . 59.301(11) ?
Ba1 Ba11 Ba1 2_655 . 118.60(2) ?
Ba1 Ba11 Ba1 3_665 . 180.0 ?
N2 Ba11 Ba1 . 4_565 45.60(18) ?
N2 Ba11 Ba1 3_665 4_565 134.40(18) ?
Ba3 Ba11 Ba1 2_655 4_565 91.665(19) ?
Ba3 Ba11 Ba1 4_565 4_565 88.335(19) ?
Ba3 Ba11 Ba1 . 4_565 120.750(18) ?
Ba3 Ba11 Ba1 3_665 4_565 59.250(18) ?
Ba12 Ba11 Ba1 1_565 4_565 59.301(11) ?
Ba12 Ba11 Ba1 . 4_565 120.699(11) ?
Ba1 Ba11 Ba1 2_655 4_565 180.0 ?
Ba1 Ba11 Ba1 3_665 4_565 118.60(2) ?
Ba1 Ba11 Ba1 . 4_565 61.40(2) ?
Ba3 Ba12 Ba3 3_655 . 180.0 ?
Ba3 Ba12 Ba3 3_655 2_655 65.04(2) ?
Ba3 Ba12 Ba3 . 2_655 114.96(2) ?
Ba3 Ba12 Ba3 3_655 4 114.96(2) ?
Ba3 Ba12 Ba3 . 4 65.04(2) ?
Ba3 Ba12 Ba3 2_655 4 180.0 ?
Ba3 Ba12 Ba9 3_655 3_655 61.230(14) ?
Ba3 Ba12 Ba9 . 3_655 118.770(14) ?
Ba3 Ba12 Ba9 2_655 3_655 61.230(14) ?
Ba3 Ba12 Ba9 4 3_655 118.770(14) ?
Ba3 Ba12 Ba9 3_655 . 118.770(14) ?
Ba3 Ba12 Ba9 . . 61.230(14) ?
Ba3 Ba12 Ba9 2_655 . 118.770(14) ?
Ba3 Ba12 Ba9 4 . 61.230(14) ?
Ba9 Ba12 Ba9 3_655 . 180.0 ?
Ba3 Ba12 Ba1 3_655 3_655 89.052(19) ?
Ba3 Ba12 Ba1 . 3_655 90.948(19) ?
Ba3 Ba12 Ba1 2_655 3_655 120.275(18) ?
Ba3 Ba12 Ba1 4 3_655 59.725(18) ?
Ba9 Ba12 Ba1 3_655 3_655 59.138(17) ?
Ba9 Ba12 Ba1 . 3_655 120.862(17) ?
Ba3 Ba12 Ba1 3_655 2_655 120.275(18) ?
Ba3 Ba12 Ba1 . 2_655 59.725(18) ?
Ba3 Ba12 Ba1 2_655 2_655 89.052(19) ?
Ba3 Ba12 Ba1 4 2_655 90.948(19) ?
Ba9 Ba12 Ba1 3_655 2_655 59.138(17) ?
Ba9 Ba12 Ba1 . 2_655 120.862(17) ?
Ba1 Ba12 Ba1 3_655 2_655 57.93(2) ?
Ba3 Ba12 Ba1 3_655 . 90.948(19) ?
Ba3 Ba12 Ba1 . . 89.052(19) ?
Ba3 Ba12 Ba1 2_655 . 59.725(18) ?
Ba3 Ba12 Ba1 4 . 120.275(18) ?
Ba9 Ba12 Ba1 3_655 . 120.862(17) ?
Ba9 Ba12 Ba1 . . 59.138(17) ?
Ba1 Ba12 Ba1 3_655 . 180.0 ?
Ba1 Ba12 Ba1 2_655 . 122.07(2) ?
Ba3 Ba12 Ba1 3_655 4 59.725(18) ?
Ba3 Ba12 Ba1 . 4 120.275(18) ?
Ba3 Ba12 Ba1 2_655 4 90.948(19) ?
Ba3 Ba12 Ba1 4 4 89.052(19) ?
Ba9 Ba12 Ba1 3_655 4 120.862(17) ?
Ba9 Ba12 Ba1 . 4 59.138(17) ?
Ba1 Ba12 Ba1 3_655 4 122.07(2) ?
Ba1 Ba12 Ba1 2_655 4 180.0 ?
Ba1 Ba12 Ba1 . 4 57.93(2) ?
Ba3 Ba12 Ba11 3_655 1_545 57.481(11) ?
Ba3 Ba12 Ba11 . 1_545 122.519(11) ?
Ba3 Ba12 Ba11 2_655 1_545 122.519(11) ?
Ba3 Ba12 Ba11 4 1_545 57.481(11) ?
Ba9 Ba12 Ba11 3_655 1_545 90.0 ?
Ba9 Ba12 Ba11 . 1_545 90.0 ?
Ba1 Ba12 Ba11 3_655 1_545 61.033(10) ?
Ba1 Ba12 Ba11 2_655 1_545 118.967(10) ?
Ba1 Ba12 Ba11 . 1_545 118.967(10) ?
Ba1 Ba12 Ba11 4 1_545 61.033(10) ?
Ba3 Ba12 Ba11 3_655 . 122.519(11) ?
Ba3 Ba12 Ba11 . . 57.481(11) ?
Ba3 Ba12 Ba11 2_655 . 57.481(11) ?
Ba3 Ba12 Ba11 4 . 122.519(11) ?
Ba9 Ba12 Ba11 3_655 . 90.0 ?
Ba9 Ba12 Ba11 . . 90.0 ?
Ba1 Ba12 Ba11 3_655 . 118.967(10) ?
Ba1 Ba12 Ba11 2_655 . 61.033(10) ?
Ba1 Ba12 Ba11 . . 61.033(10) ?
Ba1 Ba12 Ba11 4 . 118.967(10) ?
Ba11 Ba12 Ba11 1_545 . 180.0 ?
In3 In1 In2 3_666 3_566 78.17(4) ?
In3 In1 In1 3_666 4_565 56.04(2) ?
In2 In1 In1 3_566 4_565 56.153(19) ?
In3 In1 Ba6 3_666 3_556 117.30(4) ?
In2 In1 Ba6 3_566 3_556 73.82(3) ?
In1 In1 Ba6 4_565 3_556 129.977(16) ?
In3 In1 Ba5 3_666 . 89.00(3) ?
In2 In1 Ba5 3_566 . 114.24(3) ?
In1 In1 Ba5 4_565 . 63.357(14) ?
Ba6 In1 Ba5 3_556 . 153.69(3) ?
In3 In1 Ba9 3_666 3_656 73.70(3) ?
In2 In1 Ba9 3_566 3_656 118.55(4) ?
In1 In1 Ba9 4_565 3_656 129.717(17) ?
Ba6 In1 Ba9 3_556 3_656 72.78(3) ?
Ba5 In1 Ba9 . 3_656 118.55(3) ?
In3 In1 Ba4 3_666 3_566 120.56(3) ?
In2 In1 Ba4 3_566 3_566 70.24(3) ?
In1 In1 Ba4 4_565 3_566 64.526(14) ?
Ba6 In1 Ba4 3_556 3_566 100.56(3) ?
Ba5 In1 Ba4 . 3_566 62.35(2) ?
Ba9 In1 Ba4 3_656 3_566 165.46(3) ?
In3 In1 Ba8 3_666 . 122.31(4) ?
In2 In1 Ba8 3_566 . 158.20(4) ?
In1 In1 Ba8 4_565 . 126.427(15) ?
Ba6 In1 Ba8 3_556 . 99.74(3) ?
Ba5 In1 Ba8 . . 63.07(2) ?
Ba9 In1 Ba8 3_656 . 77.66(3) ?
Ba4 In1 Ba8 3_566 . 91.08(3) ?
In3 In1 Ba7 3_666 3_556 178.73(3) ?
In2 In1 Ba7 3_566 3_556 103.04(3) ?
In1 In1 Ba7 4_565 3_556 124.278(15) ?
Ba6 In1 Ba7 3_556 3_556 63.58(2) ?
Ba5 In1 Ba7 . 3_556 90.13(3) ?
Ba9 In1 Ba7 3_656 3_556 105.93(3) ?
Ba4 In1 Ba7 3_566 3_556 59.75(2) ?
Ba8 In1 Ba7 . 3_556 56.43(2) ?
In3 In1 Ba2 3_666 2_656 64.71(3) ?
In2 In1 Ba2 3_566 2_656 142.26(3) ?
In1 In1 Ba2 4_565 2_656 95.216(13) ?
Ba6 In1 Ba2 3_556 2_656 128.73(2) ?
Ba5 In1 Ba2 . 2_656 60.895(19) ?
Ba9 In1 Ba2 3_656 2_656 58.36(2) ?
Ba4 In1 Ba2 3_566 2_656 122.85(3) ?
Ba8 In1 Ba2 . 2_656 57.615(19) ?
Ba7 In1 Ba2 3_556 2_656 114.04(2) ?
In3 In1 Ba3 3_666 2_656 59.95(3) ?
In2 In1 Ba3 3_566 2_656 60.66(3) ?
In1 In1 Ba3 4_565 2_656 94.398(12) ?
Ba6 In1 Ba3 3_556 2_656 57.38(2) ?
Ba5 In1 Ba3 . 2_656 148.88(3) ?
Ba9 In1 Ba3 3_656 2_656 57.92(2) ?
Ba4 In1 Ba3 3_566 2_656 129.79(2) ?
Ba8 In1 Ba3 . 2_656 133.69(2) ?
Ba7 In1 Ba3 3_556 2_656 120.95(2) ?
Ba2 In1 Ba3 2_656 2_656 103.04(2) ?
In3 In1 Cu1 3_666 . 134.24(3) ?
In2 In1 Cu1 3_566 . 116.53(4) ?
In1 In1 Cu1 4_565 . 94.63(2) ?
Ba6 In1 Cu1 3_556 . 108.46(3) ?
Ba5 In1 Cu1 . . 45.24(2) ?
Ba9 In1 Cu1 3_656 . 122.37(3) ?
Ba4 In1 Cu1 3_566 . 46.53(2) ?
Ba8 In1 Cu1 . . 44.81(2) ?
Ba7 In1 Cu1 3_556 . 44.89(2) ?
Ba2 In1 Cu1 2_656 . 87.074(19) ?
Ba3 In1 Cu1 2_656 . 165.76(2) ?
In3 In1 In1 3_666 4 123.96(2) ?
In2 In1 In1 3_566 4 123.847(19) ?
In1 In1 In1 4_565 4 180.00(8) ?
Ba6 In1 In1 3_556 4 50.023(16) ?
Ba5 In1 In1 . 4 116.643(14) ?
Ba9 In1 In1 3_656 4 50.283(17) ?
Ba4 In1 In1 3_566 4 115.474(14) ?
Ba8 In1 In1 . 4 53.573(15) ?
Ba7 In1 In1 3_556 4 55.722(15) ?
Ba2 In1 In1 2_656 4 84.784(13) ?
Ba3 In1 In1 2_656 4 85.602(12) ?
Cu1 In1 In1 . 4 85.37(2) ?
In3 In1 N1 3_666 . 117.06(10) ?
In2 In1 N1 3_566 . 133.63(9) ?
In1 In1 N1 4_565 . 94.49(9) ?
Ba6 In1 N1 3_556 . 123.00(9) ?
Ba5 In1 N1 . . 33.06(9) ?
Ba9 In1 N1 3_656 . 107.81(9) ?
Ba4 In1 N1 3_566 . 64.44(9) ?
Ba8 In1 N1 . . 33.82(9) ?
Ba7 In1 N1 3_556 . 61.82(9) ?
Ba2 In1 N1 2_656 . 64.92(9) ?
Ba3 In1 N1 2_656 . 165.65(9) ?
Cu1 In1 N1 . . 22.23(9) ?
In1 In1 N1 4 . 85.51(9) ?
In3 In1 N1 3_666 2_556 147.07(9) ?
In2 In1 N1 3_566 2_556 98.21(9) ?
In1 In1 N1 4_565 2_556 94.46(9) ?
Ba6 In1 N1 3_556 2_556 92.26(9) ?
Ba5 In1 N1 . 2_556 62.32(9) ?
Ba9 In1 N1 3_656 2_556 132.84(9) ?
Ba4 In1 N1 3_566 2_556 33.06(9) ?
Ba8 In1 N1 . 2_556 60.76(9) ?
Ba7 In1 N1 3_556 2_556 32.63(9) ?
Ba2 In1 N1 2_656 2_556 109.02(9) ?
Ba3 In1 N1 2_656 2_556 145.73(9) ?
Cu1 In1 N1 . 2_556 22.05(8) ?
In1 In1 N1 4 2_556 85.54(9) ?
N1 In1 N1 . 2_556 44.28(16) ?
In3 In1 Ba2 3_666 2_556 129.48(3) ?
In2 In1 Ba2 3_566 2_556 51.73(2) ?
In1 In1 Ba2 4_565 2_556 94.293(10) ?
Ba6 In1 Ba2 3_556 2_556 48.745(18) ?
Ba5 In1 Ba2 . 2_556 114.90(2) ?
Ba9 In1 Ba2 3_656 2_556 121.52(2) ?
Ba4 In1 Ba2 3_566 2_556 53.136(18) ?
Ba8 In1 Ba2 . 2_556 108.20(2) ?
Ba7 In1 Ba2 3_556 2_556 51.767(17) ?
Ba2 In1 Ba2 2_656 2_556 165.81(3) ?
Ba3 In1 Ba2 2_656 2_556 86.692(17) ?
Cu1 In1 Ba2 . 2_556 81.674(16) ?
In1 In1 Ba2 4 2_556 85.707(10) ?
N1 In1 Ba2 . 2_556 103.84(9) ?
N1 In1 Ba2 2_556 2_556 59.66(9) ?
In3 In1 N5 3_666 3_656 66.85(9) ?
In2 In1 N5 3_566 3_656 135.04(14) ?
In1 In1 N5 4_565 3_656 116.94(6) ?
Ba6 In1 N5 3_556 3_656 97.51(9) ?
Ba5 In1 N5 . 3_656 93.12(12) ?
Ba9 In1 N5 3_656 3_656 25.73(11) ?
Ba4 In1 N5 3_566 3_656 152.75(14) ?
Ba8 In1 N5 . 3_656 65.75(13) ?
Ba7 In1 N5 3_556 3_656 112.28(9) ?
Ba2 In1 N5 2_656 3_656 32.63(11) ?
Ba3 In1 N5 2_656 3_656 77.31(14) ?
Cu1 In1 N5 . 3_656 108.12(14) ?
In1 In1 N5 4 3_656 63.06(6) ?
N1 In1 N5 . 3_656 88.61(16) ?
N1 In1 N5 2_556 3_656 126.51(16) ?
Ba2 In1 N5 2_556 3_656 145.57(8) ?
In3 In1 Ba2 3_666 3_666 43.21(3) ?
In2 In1 Ba2 3_566 3_666 101.17(3) ?
In1 In1 Ba2 4_565 3_666 48.891(13) ?
Ba6 In1 Ba2 3_556 3_666 160.04(3) ?
Ba5 In1 Ba2 . 3_666 46.077(17) ?
Ba9 In1 Ba2 3_656 3_666 93.85(2) ?
Ba4 In1 Ba2 3_566 3_666 95.63(2) ?
Ba8 In1 Ba2 . 3_666 91.49(2) ?
Ba7 In1 Ba2 3_556 3_666 135.83(2) ?
Ba2 In1 Ba2 2_656 3_666 46.325(18) ?
Ba3 In1 Ba2 2_656 3_666 103.083(19) ?
Cu1 In1 Ba2 . 3_666 91.15(2) ?
In1 In1 Ba2 4 3_666 131.110(13) ?
N1 In1 Ba2 . 3_666 74.70(9) ?
N1 In1 Ba2 2_556 3_666 107.64(9) ?
Ba2 In1 Ba2 2_556 3_666 141.986(18) ?
N5 In1 Ba2 3_656 3_666 72.05(7) ?
In3 In1 Ba3 3_666 3_666 39.01(2) ?
In2 In1 Ba3 3_566 3_666 39.85(3) ?
In1 In1 Ba3 4_565 3_666 49.749(13) ?
Ba6 In1 Ba3 3_556 3_666 92.31(2) ?
Ba5 In1 Ba3 . 3_666 109.83(2) ?
Ba9 In1 Ba3 3_656 3_666 92.52(3) ?
Ba4 In1 Ba3 3_566 3_666 100.76(2) ?
Ba8 In1 Ba3 . 3_666 161.31(3) ?
Ba7 In1 Ba3 3_556 3_666 142.25(2) ?
Ba2 In1 Ba3 2_656 3_666 103.69(2) ?
Ba3 In1 Ba3 2_656 3_666 44.649(17) ?
Cu1 In1 Ba3 . 3_666 143.02(3) ?
In1 In1 Ba3 4 3_666 130.251(13) ?
N1 In1 Ba3 . 3_666 142.83(9) ?
N1 In1 Ba3 2_556 3_666 133.42(9) ?
Ba2 In1 Ba3 2_556 3_666 90.492(15) ?
N5 In1 Ba3 3_656 3_666 98.69(12) ?
Ba2 In1 Ba3 3_666 3_666 73.133(16) ?
In3 In1 Ba1 3_666 2_556 92.99(3) ?
In2 In1 Ba1 3_566 2_556 38.702(18) ?
In1 In1 Ba1 4_565 2_556 94.108(9) ?
Ba6 In1 Ba1 3_556 2_556 36.625(14) ?
Ba5 In1 Ba1 . 2_556 150.95(2) ?
Ba9 In1 Ba1 3_656 2_556 89.68(2) ?
Ba4 In1 Ba1 3_566 2_556 92.18(2) ?
Ba8 In1 Ba1 . 2_556 135.92(2) ?
Ba7 In1 Ba1 3_556 2_556 88.22(2) ?
Ba2 In1 Ba1 2_656 2_556 144.29(2) ?
Ba3 In1 Ba1 2_656 2_556 41.823(15) ?
Cu1 In1 Ba1 . 2_556 126.37(2) ?
In1 In1 Ba1 4 2_556 85.892(9) ?
N1 In1 Ba1 . 2_556 148.18(9) ?
N1 In1 Ba1 2_556 2_556 104.50(9) ?
Ba2 In1 Ba1 2_556 2_556 44.935(15) ?
N5 In1 Ba1 3_656 2_556 114.28(13) ?
Ba2 In1 Ba1 3_666 2_556 131.786(18) ?
Ba3 In1 Ba1 3_666 2_556 58.671(15) ?
In1 In2 In1 2_556 3_566 67.69(4) ?
In1 In2 In3 2_556 1_455 50.82(3) ?
In1 In2 In3 3_566 1_455 50.82(3) ?
In1 In2 Ba3 2_556 1_455 77.15(3) ?
In1 In2 Ba3 3_566 1_455 110.56(4) ?
In3 In2 Ba3 1_455 1_455 60.32(3) ?
In1 In2 Ba3 2_556 4_465 110.56(4) ?
In1 In2 Ba3 3_566 4_465 77.15(3) ?
In3 In2 Ba3 1_455 4_465 60.32(3) ?
Ba3 In2 Ba3 1_455 4_465 61.99(3) ?
In1 In2 Ba4 2_556 . 65.24(3) ?
In1 In2 Ba4 3_566 . 65.24(3) ?
In3 In2 Ba4 1_455 . 100.18(3) ?
Ba3 In2 Ba4 1_455 . 140.92(2) ?
Ba3 In2 Ba4 4_465 . 140.92(2) ?
In1 In2 Ba6 2_556 1_565 128.80(3) ?
In1 In2 Ba6 3_566 1_565 61.10(2) ?
In3 In2 Ba6 1_455 1_565 93.84(2) ?
Ba3 In2 Ba6 1_455 1_565 120.54(3) ?
Ba3 In2 Ba6 4_465 1_565 58.812(19) ?
Ba4 In2 Ba6 . 1_565 92.39(2) ?
In1 In2 Ba6 2_556 . 61.10(2) ?
In1 In2 Ba6 3_566 . 128.80(3) ?
In3 In2 Ba6 1_455 . 93.84(2) ?
Ba3 In2 Ba6 1_455 . 58.812(19) ?
Ba3 In2 Ba6 4_465 . 120.54(3) ?
Ba4 In2 Ba6 . . 92.39(2) ?
Ba6 In2 Ba6 1_565 . 170.10(4) ?
In1 In2 Ba1 2_556 4_565 168.08(4) ?
In1 In2 Ba1 3_566 4_565 113.92(2) ?
In3 In2 Ba1 1_455 4_565 120.12(3) ?
Ba3 In2 Ba1 1_455 4_565 91.53(3) ?
Ba3 In2 Ba1 4_465 4_565 59.80(2) ?
Ba4 In2 Ba1 . 4_565 126.56(3) ?
Ba6 In2 Ba1 1_565 4_565 54.275(16) ?
Ba6 In2 Ba1 . 4_565 116.17(3) ?
In1 In2 Ba1 2_556 . 113.92(2) ?
In1 In2 Ba1 3_566 . 168.08(4) ?
In3 In2 Ba1 1_455 . 120.12(3) ?
Ba3 In2 Ba1 1_455 . 59.80(2) ?
Ba3 In2 Ba1 4_465 . 91.53(3) ?
Ba4 In2 Ba1 . . 126.56(3) ?
Ba6 In2 Ba1 1_565 . 116.17(3) ?
Ba6 In2 Ba1 . . 54.275(16) ?
Ba1 In2 Ba1 4_565 . 61.91(3) ?
In1 In2 Ba2 2_556 4_565 128.02(4) ?
In1 In2 Ba2 3_566 4_565 93.22(3) ?
In3 In2 Ba2 1_455 4_565 143.48(2) ?
Ba3 In2 Ba2 1_455 4_565 151.60(3) ?
Ba3 In2 Ba2 4_465 4_565 111.23(2) ?
Ba4 In2 Ba2 . 4_565 62.89(2) ?
Ba6 In2 Ba2 1_565 4_565 57.503(19) ?
Ba6 In2 Ba2 . 4_565 117.65(3) ?
Ba1 In2 Ba2 4_565 4_565 63.88(2) ?
Ba1 In2 Ba2 . 4_565 94.40(3) ?
In1 In2 Ba2 2_556 . 93.22(3) ?
In1 In2 Ba2 3_566 . 128.02(4) ?
In3 In2 Ba2 1_455 . 143.48(2) ?
Ba3 In2 Ba2 1_455 . 111.23(2) ?
Ba3 In2 Ba2 4_465 . 151.60(3) ?
Ba4 In2 Ba2 . . 62.89(2) ?
Ba6 In2 Ba2 1_565 . 117.65(3) ?
Ba6 In2 Ba2 . . 57.503(19) ?
Ba1 In2 Ba2 4_565 . 94.40(3) ?
Ba1 In2 Ba2 . . 63.88(2) ?
Ba2 In2 Ba2 4_565 . 60.34(3) ?
In1 In2 Cu2 2_556 . 120.92(3) ?
In1 In2 Cu2 3_566 . 120.92(3) ?
In3 In2 Cu2 1_455 . 87.76(3) ?
Ba3 In2 Cu2 1_455 . 44.058(17) ?
Ba3 In2 Cu2 4_465 . 44.058(17) ?
Ba4 In2 Cu2 . . 172.06(3) ?
Ba6 In2 Cu2 1_565 . 87.04(2) ?
Ba6 In2 Cu2 . . 87.04(2) ?
Ba1 In2 Cu2 4_565 . 47.531(17) ?
Ba1 In2 Cu2 . . 47.531(17) ?
Ba2 In2 Cu2 4_565 . 110.48(2) ?
Ba2 In2 Cu2 . . 110.48(2) ?
In1 In2 N3 2_556 . 94.31(13) ?
In1 In2 N3 3_566 . 94.31(13) ?
In3 In2 N3 1_455 . 135.66(15) ?
Ba3 In2 N3 1_455 . 147.48(4) ?
Ba3 In2 N3 4_465 . 147.48(4) ?
Ba4 In2 N3 . . 35.48(15) ?
Ba6 In2 N3 1_565 . 89.43(3) ?
Ba6 In2 N3 . . 89.43(3) ?
Ba1 In2 N3 4_565 . 97.30(13) ?
Ba1 In2 N3 . . 97.30(13) ?
Ba2 In2 N3 4_565 . 37.11(8) ?
Ba2 In2 N3 . . 37.11(8) ?
Cu2 In2 N3 . . 136.58(15) ?
In1 In2 N4 2_556 . 81.26(12) ?
In1 In2 N4 3_566 . 139.70(14) ?
In3 In2 N4 1_455 . 89.78(14) ?
Ba3 In2 N4 1_455 . 34.50(14) ?
Ba3 In2 N4 4_465 . 91.22(13) ?
Ba4 In2 N4 . . 124.24(12) ?
Ba6 In2 N4 1_565 . 141.92(12) ?
Ba6 In2 N4 . . 31.93(12) ?
Ba1 In2 N4 4_565 . 91.56(12) ?
Ba1 In2 N4 . . 35.17(13) ?
Ba2 In2 N4 4_565 . 126.69(14) ?
Ba2 In2 N4 . . 76.84(14) ?
Cu2 In2 N4 . . 55.21(12) ?
N3 In2 N4 . . 113.68(15) ?
In1 In2 N4 2_556 1_565 139.70(14) ?
In1 In2 N4 3_566 1_565 81.26(12) ?
In3 In2 N4 1_455 1_565 89.78(14) ?
Ba3 In2 N4 1_455 1_565 91.22(13) ?
Ba3 In2 N4 4_465 1_565 34.50(14) ?
Ba4 In2 N4 . 1_565 124.24(12) ?
Ba6 In2 N4 1_565 1_565 31.93(12) ?
Ba6 In2 N4 . 1_565 141.92(12) ?
Ba1 In2 N4 4_565 1_565 35.17(13) ?
Ba1 In2 N4 . 1_565 91.56(12) ?
Ba2 In2 N4 4_565 1_565 76.84(14) ?
Ba2 In2 N4 . 1_565 126.69(14) ?
Cu2 In2 N4 . 1_565 55.21(12) ?
N3 In2 N4 . 1_565 113.68(15) ?
N4 In2 N4 . 1_565 110.4(2) ?
In1 In2 N5 2_556 1_565 152.09(14) ?
In1 In2 N5 3_566 1_565 88.90(11) ?
In3 In2 N5 1_455 1_565 124.77(11) ?
Ba3 In2 N5 1_455 1_565 127.33(15) ?
Ba3 In2 N5 4_465 1_565 76.80(14) ?
Ba4 In2 N5 . 1_565 91.75(15) ?
Ba6 In2 N5 1_565 1_565 31.46(11) ?
Ba6 In2 N5 . 1_565 139.64(11) ?
Ba1 In2 N5 4_565 1_565 37.26(14) ?
Ba1 In2 N5 . 1_565 92.17(12) ?
Ba2 In2 N5 4_565 1_565 34.60(15) ?
Ba2 In2 N5 . 1_565 89.51(13) ?
Cu2 In2 N5 . 1_565 83.63(15) ?
N3 In2 N5 . 1_565 71.66(17) ?
N4 In2 N5 . 1_565 126.26(17) ?
N4 In2 N5 1_565 1_565 42.3(2) ?
In1 In2 N5 2_556 . 88.90(11) ?
In1 In2 N5 3_566 . 152.09(14) ?
In3 In2 N5 1_455 . 124.77(11) ?
Ba3 In2 N5 1_455 . 76.80(15) ?
Ba3 In2 N5 4_465 . 127.33(15) ?
Ba4 In2 N5 . . 91.75(15) ?
Ba6 In2 N5 1_565 . 139.64(11) ?
Ba6 In2 N5 . . 31.46(11) ?
Ba1 In2 N5 4_565 . 92.17(12) ?
Ba1 In2 N5 . . 37.26(14) ?
Ba2 In2 N5 4_565 . 89.51(13) ?
Ba2 In2 N5 . . 34.60(15) ?
Cu2 In2 N5 . . 83.63(15) ?
N3 In2 N5 . . 71.66(17) ?
N4 In2 N5 . . 42.3(2) ?
N4 In2 N5 1_565 . 126.26(17) ?
N5 In2 N5 1_565 . 108.3(2) ?
In1 In2 N2 2_556 3_565 103.00(10) ?
In1 In2 N2 3_566 3_565 103.00(10) ?
In3 In2 N2 1_455 3_565 65.25(12) ?
Ba3 In2 N2 1_455 3_565 32.56(4) ?
Ba3 In2 N2 4_465 3_565 32.56(4) ?
Ba4 In2 N2 . 3_565 165.43(12) ?
Ba6 In2 N2 1_565 3_565 88.78(2) ?
Ba6 In2 N2 . 3_565 88.78(2) ?
Ba1 In2 N2 4_565 3_565 65.08(10) ?
Ba1 In2 N2 . 3_565 65.08(10) ?
Ba2 In2 N2 4_565 3_565 128.75(9) ?
Ba2 In2 N2 . 3_565 128.75(9) ?
Cu2 In2 N2 . 3_565 22.51(12) ?
N3 In2 N2 . 3_565 159.09(19) ?
N4 In2 N2 . 3_565 58.66(13) ?
N4 In2 N2 1_565 3_565 58.67(13) ?
N5 In2 N2 1_565 3_565 96.76(17) ?
N5 In2 N2 . 3_565 96.76(17) ?
In1 In2 N2 2_556 . 136.07(8) ?
In1 In2 N2 3_566 . 136.07(8) ?
In3 In2 N2 1_455 . 109.66(13) ?
Ba3 In2 N2 1_455 . 60.50(10) ?
Ba3 In2 N2 4_465 . 60.50(10) ?
Ba4 In2 N2 . . 150.16(13) ?
Ba6 In2 N2 1_565 . 85.77(2) ?
Ba6 In2 N2 . . 85.77(2) ?
Ba1 In2 N2 4_565 . 34.54(5) ?
Ba1 In2 N2 . . 34.54(5) ?
Ba2 In2 N2 4_565 . 91.70(11) ?
Ba2 In2 N2 . . 91.70(11) ?
Cu2 In2 N2 . . 21.91(13) ?
N3 In2 N2 . . 114.7(2) ?
N4 In2 N2 . . 57.56(12) ?
N4 In2 N2 1_565 . 57.56(12) ?
N5 In2 N2 1_565 . 71.49(15) ?
N5 In2 N2 . . 71.49(15) ?
N2 In2 N2 3_565 . 44.4(2) ?
In1 In3 In1 3_666 2_656 67.91(4) ?
In1 In3 In2 3_666 1_655 51.02(3) ?
In1 In3 In2 2_656 1_655 51.02(3) ?
In1 In3 Ba3 3_666 . 111.76(4) ?
In1 In3 Ba3 2_656 . 77.86(3) ?
In2 In3 Ba3 1_655 . 61.33(2) ?
In1 In3 Ba3 3_666 4_565 77.86(3) ?
In1 In3 Ba3 2_656 4_565 111.76(4) ?
In2 In3 Ba3 1_655 4_565 61.33(2) ?
Ba3 In3 Ba3 . 4_565 62.67(3) ?
In1 In3 Ba2 3_666 4_565 73.41(3) ?
In1 In3 Ba2 2_656 4_565 106.43(4) ?
In2 In3 Ba2 1_655 4_565 124.05(3) ?
Ba3 In3 Ba2 . 4_565 174.46(4) ?
Ba3 In3 Ba2 4_565 4_565 117.788(18) ?
In1 In3 Ba2 3_666 . 106.43(4) ?
In1 In3 Ba2 2_656 . 73.41(3) ?
In2 In3 Ba2 1_655 . 124.05(3) ?
Ba3 In3 Ba2 . . 117.788(18) ?
Ba3 In3 Ba2 4_565 . 174.46(4) ?
Ba2 In3 Ba2 4_565 . 61.16(3) ?
In1 In3 Ba9 3_666 . 129.37(4) ?
In1 In3 Ba9 2_656 . 61.49(2) ?
In2 In3 Ba9 1_655 . 95.11(2) ?
Ba3 In3 Ba9 . . 59.726(17) ?
Ba3 In3 Ba9 4_565 . 122.06(3) ?
Ba2 In3 Ba9 4_565 . 118.92(3) ?
Ba2 In3 Ba9 . . 58.063(18) ?
In1 In3 Ba9 3_666 1_565 61.49(2) ?
In1 In3 Ba9 2_656 1_565 129.37(4) ?
In2 In3 Ba9 1_655 1_565 95.11(2) ?
Ba3 In3 Ba9 . 1_565 122.06(3) ?
Ba3 In3 Ba9 4_565 1_565 59.726(17) ?
Ba2 In3 Ba9 4_565 1_565 58.063(18) ?
Ba2 In3 Ba9 . 1_565 118.92(3) ?
Ba9 In3 Ba9 . 1_565 168.72(4) ?
In1 In3 Ba11 3_666 . 133.18(3) ?
In1 In3 Ba11 2_656 . 133.18(3) ?
In2 In3 Ba11 1_655 . 104.91(3) ?
Ba3 In3 Ba11 . . 55.99(2) ?
Ba3 In3 Ba11 4_565 . 55.99(2) ?
Ba2 In3 Ba11 4_565 . 119.20(3) ?
Ba2 In3 Ba11 . . 119.20(3) ?
Ba9 In3 Ba11 . . 86.38(2) ?
Ba9 In3 Ba11 1_565 . 86.38(2) ?
In1 In3 Ba1 3_666 . 164.07(4) ?
In1 In3 Ba1 2_656 . 115.09(2) ?
In2 In3 Ba1 1_655 . 143.79(3) ?
Ba3 In3 Ba1 . . 83.96(3) ?
Ba3 In3 Ba1 4_565 . 113.29(4) ?
Ba2 In3 Ba1 4_565 . 90.98(3) ?
Ba2 In3 Ba1 . . 61.80(2) ?
Ba9 In3 Ba1 . . 55.597(18) ?
Ba9 In3 Ba1 1_565 . 113.13(3) ?
Ba11 In3 Ba1 . . 57.408(19) ?
In1 In3 Ba1 3_666 4_565 115.09(2) ?
In1 In3 Ba1 2_656 4_565 164.07(4) ?
In2 In3 Ba1 1_655 4_565 143.79(3) ?
Ba3 In3 Ba1 . 4_565 113.29(4) ?
Ba3 In3 Ba1 4_565 4_565 83.96(3) ?
Ba2 In3 Ba1 4_565 4_565 61.80(2) ?
Ba2 In3 Ba1 . 4_565 90.98(3) ?
Ba9 In3 Ba1 . 4_565 113.13(3) ?
Ba9 In3 Ba1 1_565 4_565 55.597(18) ?
Ba11 In3 Ba1 . 4_565 57.408(19) ?
Ba1 In3 Ba1 . 4_565 57.53(3) ?
In1 In3 Ba5 3_666 3_666 51.85(3) ?
In1 In3 Ba5 2_656 3_666 51.85(3) ?
In2 In3 Ba5 1_655 3_666 82.53(3) ?
Ba3 In3 Ba5 . 3_666 129.67(3) ?
Ba3 In3 Ba5 4_565 3_666 129.67(3) ?
Ba2 In3 Ba5 4_565 3_666 54.85(2) ?
Ba2 In3 Ba5 . 3_666 54.85(2) ?
Ba9 In3 Ba5 . 3_666 93.03(2) ?
Ba9 In3 Ba5 1_565 3_666 93.03(2) ?
Ba11 In3 Ba5 . 3_666 172.55(3) ?
Ba1 In3 Ba5 . 3_666 116.39(3) ?
Ba1 In3 Ba5 4_565 3_666 116.39(3) ?
In1 In3 N2 3_666 3_665 107.00(12) ?
In1 In3 N2 2_656 3_665 107.00(12) ?
In2 In3 N2 1_655 3_665 69.97(14) ?
Ba3 In3 N2 . 3_665 34.08(5) ?
Ba3 In3 N2 4_565 3_665 34.08(5) ?
Ba2 In3 N2 4_565 3_665 143.73(7) ?
Ba2 In3 N2 . 3_665 143.73(7) ?
Ba9 In3 N2 . 3_665 89.51(2) ?
Ba9 In3 N2 1_565 3_665 89.51(2) ?
Ba11 In3 N2 . 3_665 34.95(14) ?
Ba1 In3 N2 . 3_665 87.40(12) ?
Ba1 In3 N2 4_565 3_665 87.40(12) ?
Ba5 In3 N2 3_666 3_665 152.50(14) ?
In1 In3 N5 3_666 . 137.07(16) ?
In1 In3 N5 2_656 . 79.19(14) ?
In2 In3 N5 1_655 . 123.42(12) ?
Ba3 In3 N5 . . 86.16(12) ?
Ba3 In3 N5 4_565 . 142.12(15) ?
Ba2 In3 N5 4_565 . 91.19(12) ?
Ba2 In3 N5 . . 35.22(14) ?
Ba9 In3 N5 . . 30.38(11) ?
Ba9 In3 N5 1_565 . 140.89(11) ?
Ba11 In3 N5 . . 89.47(16) ?
Ba1 In3 N5 . . 37.47(15) ?
Ba1 In3 N5 4_565 . 89.93(13) ?
Ba5 In3 N5 3_666 . 86.31(15) ?
N2 In3 N5 3_665 . 108.51(16) ?
In1 In3 N5 3_666 1_565 79.19(14) ?
In1 In3 N5 2_656 1_565 137.07(16) ?
In2 In3 N5 1_655 1_565 123.42(12) ?
Ba3 In3 N5 . 1_565 142.12(15) ?
Ba3 In3 N5 4_565 1_565 86.16(12) ?
Ba2 In3 N5 4_565 1_565 35.22(14) ?
Ba2 In3 N5 . 1_565 91.19(12) ?
Ba9 In3 N5 . 1_565 140.89(11) ?
Ba9 In3 N5 1_565 1_565 30.38(11) ?
Ba11 In3 N5 . 1_565 89.47(16) ?
Ba1 In3 N5 . 1_565 89.93(13) ?
Ba1 In3 N5 4_565 1_565 37.47(15) ?
Ba5 In3 N5 3_666 1_565 86.31(15) ?
N2 In3 N5 3_665 1_565 108.51(16) ?
N5 In3 N5 . 1_565 110.8(2) ?
In1 In3 N3 3_666 . 76.64(13) ?
In1 In3 N3 2_656 . 76.64(13) ?
In2 In3 N3 1_655 . 114.50(16) ?
Ba3 In3 N3 . . 147.35(4) ?
Ba3 In3 N3 4_565 . 147.35(5) ?
Ba2 In3 N3 4_565 . 34.18(7) ?
Ba2 In3 N3 . . 34.18(7) ?
Ba9 In3 N3 . . 90.05(3) ?
Ba9 In3 N3 1_565 . 90.05(3) ?
Ba11 In3 N3 . . 140.59(16) ?
Ba1 In3 N3 . . 88.69(14) ?
Ba1 In3 N3 4_565 . 88.69(14) ?
Ba5 In3 N3 3_666 . 31.96(16) ?
N2 In3 N3 3_665 . 175.5(2) ?
N5 In3 N3 . . 69.32(16) ?
N5 In3 N3 1_565 . 69.32(16) ?
In1 In3 N2 3_666 . 145.99(2) ?
In1 In3 N2 2_656 . 145.99(2) ?
In2 In3 N2 1_655 . 137.34(12) ?
Ba3 In3 N2 . . 82.75(10) ?
Ba3 In3 N2 4_565 . 82.75(10) ?
Ba2 In3 N2 4_565 . 91.80(10) ?
Ba2 In3 N2 . . 91.80(10) ?
Ba9 In3 N2 . . 84.63(2) ?
Ba9 In3 N2 1_565 . 84.63(2) ?
Ba11 In3 N2 . . 32.42(12) ?
Ba1 In3 N2 . . 34.36(6) ?
Ba1 In3 N2 4_565 . 34.36(6) ?
Ba5 In3 N2 3_666 . 140.13(12) ?
N2 In3 N2 3_665 . 67.4(2) ?
N5 In3 N2 . . 71.82(16) ?
N5 In3 N2 1_565 . 71.82(16) ?
N3 In3 N2 . . 108.2(2) ?
In1 In3 In2 3_666 . 119.00(3) ?
In1 In3 In2 2_656 . 119.00(3) ?
In2 In3 In2 1_655 . 166.43(4) ?
Ba3 In3 In2 . . 129.21(3) ?
Ba3 In3 In2 4_565 . 129.21(3) ?
Ba2 In3 In2 4_565 . 45.759(18) ?
Ba2 In3 In2 . . 45.759(18) ?
Ba9 In3 In2 . . 85.593(19) ?
Ba9 In3 In2 1_565 . 85.593(19) ?
Ba11 In3 In2 . . 88.65(3) ?
Ba1 In3 In2 . . 45.248(19) ?
Ba1 In3 In2 4_565 . 45.248(19) ?
Ba5 In3 In2 3_666 . 83.90(2) ?
N2 In3 In2 3_665 . 123.60(14) ?
N5 In3 In2 . . 55.42(11) ?
N5 In3 In2 1_565 . 55.42(11) ?
N3 In3 In2 . . 51.94(16) ?
N2 In3 In2 . . 56.23(12) ?
In1 In3 Ba6 3_666 1_665 35.08(2) ?
In1 In3 Ba6 2_656 1_665 88.36(3) ?
In2 In3 Ba6 1_655 1_665 45.071(13) ?
Ba3 In3 Ba6 . 1_665 90.09(2) ?
Ba3 In3 Ba6 4_565 1_665 42.804(17) ?
Ba2 In3 Ba6 4_565 1_665 93.50(2) ?
Ba2 In3 Ba6 . 1_665 141.29(3) ?
Ba9 In3 Ba6 . 1_665 139.89(3) ?
Ba9 In3 Ba6 1_565 1_665 50.043(18) ?
Ba11 In3 Ba6 . 1_665 98.309(19) ?
Ba1 In3 Ba6 . 1_665 153.75(3) ?
Ba1 In3 Ba6 4_565 1_665 102.501(19) ?
Ba5 In3 Ba6 3_666 1_665 86.93(2) ?
N2 In3 Ba6 3_665 1_665 73.85(9) ?
N5 In3 Ba6 . 1_665 167.50(14) ?
N5 In3 Ba6 1_565 1_665 79.18(11) ?
N3 In3 Ba6 . 1_665 109.14(11) ?
N2 In3 Ba6 . 1_665 119.55(7) ?
In2 In3 Ba6 . 1_665 134.072(14) ?
N1 Cu1 Ba5 2_556 . 124.2(2) ?
N1 Cu1 Ba5 . . 56.5(2) ?
N1 Cu1 Ba5 2_556 3_566 56.5(2) ?
N1 Cu1 Ba5 . 3_566 124.2(2) ?
Ba5 Cu1 Ba5 . 3_566 104.90(5) ?
N1 Cu1 Ba8 2_556 3_556 56.5(2) ?
N1 Cu1 Ba8 . 3_556 122.7(2) ?
Ba5 Cu1 Ba8 . 3_556 178.03(3) ?
Ba5 Cu1 Ba8 3_566 3_556 73.90(2) ?
N1 Cu1 Ba8 2_556 . 122.7(2) ?
N1 Cu1 Ba8 . . 56.5(2) ?
Ba5 Cu1 Ba8 . . 73.90(2) ?
Ba5 Cu1 Ba8 3_566 . 178.03(3) ?
Ba8 Cu1 Ba8 3_556 . 107.34(5) ?
N1 Cu1 Ba7 2_556 . 126.3(2) ?
N1 Cu1 Ba7 . . 53.0(2) ?
Ba5 Cu1 Ba7 . . 109.48(2) ?
Ba5 Cu1 Ba7 3_566 . 112.14(2) ?
Ba8 Cu1 Ba7 3_556 . 69.80(3) ?
Ba8 Cu1 Ba7 . . 69.80(3) ?
N1 Cu1 Ba7 2_556 3_556 53.0(2) ?
N1 Cu1 Ba7 . 3_556 126.3(2) ?
Ba5 Cu1 Ba7 . 3_556 112.14(2) ?
Ba5 Cu1 Ba7 3_566 3_556 109.48(2) ?
Ba8 Cu1 Ba7 3_556 3_556 69.80(3) ?
Ba8 Cu1 Ba7 . 3_556 69.80(3) ?
Ba7 Cu1 Ba7 . 3_556 108.71(5) ?
N1 Cu1 Ba4 2_556 . 126.9(2) ?
N1 Cu1 Ba4 . . 53.8(2) ?
Ba5 Cu1 Ba4 . . 67.42(3) ?
Ba5 Cu1 Ba4 3_566 . 70.39(3) ?
Ba8 Cu1 Ba4 3_556 . 110.63(2) ?
Ba8 Cu1 Ba4 . . 110.30(2) ?
Ba7 Cu1 Ba4 . . 71.815(18) ?
Ba7 Cu1 Ba4 3_556 . 179.44(4) ?
N1 Cu1 Ba4 2_556 3_566 53.8(2) ?
N1 Cu1 Ba4 . 3_566 126.9(2) ?
Ba5 Cu1 Ba4 . 3_566 70.39(3) ?
Ba5 Cu1 Ba4 3_566 3_566 67.42(3) ?
Ba8 Cu1 Ba4 3_556 3_566 110.30(2) ?
Ba8 Cu1 Ba4 . 3_566 110.63(2) ?
Ba7 Cu1 Ba4 . 3_566 179.44(4) ?
Ba7 Cu1 Ba4 3_556 3_566 71.815(18) ?
Ba4 Cu1 Ba4 . 3_566 107.66(5) ?
N1 Cu1 In1 2_556 . 90.7(3) ?
N1 Cu1 In1 . . 89.4(3) ?
Ba5 Cu1 In1 . . 51.850(17) ?
Ba5 Cu1 In1 3_566 . 121.29(3) ?
Ba8 Cu1 In1 3_556 . 130.09(3) ?
Ba8 Cu1 In1 . . 56.747(18) ?
Ba7 Cu1 In1 . . 126.14(3) ?
Ba7 Cu1 In1 3_556 . 60.29(2) ?
Ba4 Cu1 In1 . . 119.27(3) ?
Ba4 Cu1 In1 3_566 . 54.255(19) ?
N1 Cu1 In1 2_556 2_556 89.4(3) ?
N1 Cu1 In1 . 2_556 90.7(3) ?
Ba5 Cu1 In1 . 2_556 121.29(3) ?
Ba5 Cu1 In1 3_566 2_556 51.850(17) ?
Ba8 Cu1 In1 3_556 2_556 56.747(18) ?
Ba8 Cu1 In1 . 2_556 130.09(3) ?
Ba7 Cu1 In1 . 2_556 60.29(2) ?
Ba7 Cu1 In1 3_556 2_556 126.14(3) ?
Ba4 Cu1 In1 . 2_556 54.255(19) ?
Ba4 Cu1 In1 3_566 2_556 119.27(3) ?
In1 Cu1 In1 . 2_556 170.74(4) ?
N2 Cu2 Ba3 3_565 2_655 124.7(2) ?
N2 Cu2 Ba3 . 2_655 55.3(2) ?
N2 Cu2 Ba3 3_565 3_665 124.7(2) ?
N2 Cu2 Ba3 . 3_665 55.3(2) ?
Ba3 Cu2 Ba3 2_655 3_665 74.21(2) ?
N2 Cu2 Ba3 3_565 1_455 55.3(2) ?
N2 Cu2 Ba3 . 1_455 124.7(2) ?
Ba3 Cu2 Ba3 2_655 1_455 105.79(2) ?
Ba3 Cu2 Ba3 3_665 1_455 180.0 ?
N2 Cu2 Ba3 3_565 4_465 55.3(2) ?
N2 Cu2 Ba3 . 4_465 124.7(2) ?
Ba3 Cu2 Ba3 2_655 4_465 180.0 ?
Ba3 Cu2 Ba3 3_665 4_465 105.79(2) ?
Ba3 Cu2 Ba3 1_455 4_465 74.21(2) ?
N2 Cu2 Ba1 3_565 2 54.6(3) ?
N2 Cu2 Ba1 . 2 125.4(3) ?
Ba3 Cu2 Ba1 2_655 2 70.03(2) ?
Ba3 Cu2 Ba1 3_665 2 111.24(2) ?
Ba3 Cu2 Ba1 1_455 2 68.76(2) ?
Ba3 Cu2 Ba1 4_465 2 109.97(2) ?
N2 Cu2 Ba1 3_565 4_565 125.4(3) ?
N2 Cu2 Ba1 . 4_565 54.6(3) ?
Ba3 Cu2 Ba1 2_655 4_565 109.97(2) ?
Ba3 Cu2 Ba1 3_665 4_565 68.76(2) ?
Ba3 Cu2 Ba1 1_455 4_565 111.24(2) ?
Ba3 Cu2 Ba1 4_465 4_565 70.03(2) ?
Ba1 Cu2 Ba1 2 4_565 180.0 ?
N2 Cu2 Ba1 3_565 3_565 54.6(3) ?
N2 Cu2 Ba1 . 3_565 125.4(3) ?
Ba3 Cu2 Ba1 2_655 3_565 111.24(2) ?
Ba3 Cu2 Ba1 3_665 3_565 70.03(2) ?
Ba3 Cu2 Ba1 1_455 3_565 109.97(2) ?
Ba3 Cu2 Ba1 4_465 3_565 68.76(2) ?
Ba1 Cu2 Ba1 2 3_565 71.37(2) ?
Ba1 Cu2 Ba1 4_565 3_565 108.63(2) ?
N2 Cu2 Ba1 3_565 . 125.4(3) ?
N2 Cu2 Ba1 . . 54.6(3) ?
Ba3 Cu2 Ba1 2_655 . 68.76(2) ?
Ba3 Cu2 Ba1 3_665 . 109.97(2) ?
Ba3 Cu2 Ba1 1_455 . 70.03(2) ?
Ba3 Cu2 Ba1 4_465 . 111.24(2) ?
Ba1 Cu2 Ba1 2 . 108.63(2) ?
Ba1 Cu2 Ba1 4_565 . 71.37(2) ?
Ba1 Cu2 Ba1 3_565 . 180.0 ?
N2 Cu2 In2 3_565 3_565 92.1(4) ?
N2 Cu2 In2 . 3_565 87.9(4) ?
Ba3 Cu2 In2 2_655 3_565 54.556(16) ?
Ba3 Cu2 In2 3_665 3_565 54.556(16) ?
Ba3 Cu2 In2 1_455 3_565 125.444(16) ?
Ba3 Cu2 In2 4_465 3_565 125.444(16) ?
Ba1 Cu2 In2 2 3_565 56.767(16) ?
Ba1 Cu2 In2 4_565 3_565 123.233(16) ?
Ba1 Cu2 In2 3_565 3_565 56.767(16) ?
Ba1 Cu2 In2 . 3_565 123.233(16) ?
N2 Cu2 In2 3_565 . 87.9(4) ?
N2 Cu2 In2 . . 92.1(4) ?
Ba3 Cu2 In2 2_655 . 125.444(16) ?
Ba3 Cu2 In2 3_665 . 125.444(16) ?
Ba3 Cu2 In2 1_455 . 54.556(16) ?
Ba3 Cu2 In2 4_465 . 54.556(16) ?
Ba1 Cu2 In2 2 . 123.233(16) ?
Ba1 Cu2 In2 4_565 . 56.767(16) ?
Ba1 Cu2 In2 3_565 . 123.233(16) ?
Ba1 Cu2 In2 . . 56.767(16) ?
In2 Cu2 In2 3_565 . 180.0 ?
N4 Cu3 Ba3 3 3_655 56.7(2) ?
N4 Cu3 Ba3 . 3_655 123.3(2) ?
N4 Cu3 Ba3 3 2_655 56.7(2) ?
N4 Cu3 Ba3 . 2_655 123.3(2) ?
Ba3 Cu3 Ba3 3_655 2_655 75.42(2) ?
N4 Cu3 Ba3 3 4_455 123.3(2) ?
N4 Cu3 Ba3 . 4_455 56.7(2) ?
Ba3 Cu3 Ba3 3_655 4_455 104.58(2) ?
Ba3 Cu3 Ba3 2_655 4_455 180.0 ?
N4 Cu3 Ba3 3 1_455 123.3(2) ?
N4 Cu3 Ba3 . 1_455 56.7(2) ?
Ba3 Cu3 Ba3 3_655 1_455 180.0 ?
Ba3 Cu3 Ba3 2_655 1_455 104.58(2) ?
Ba3 Cu3 Ba3 4_455 1_455 75.42(2) ?
N4 Cu3 Ba1 3 3 53.9(3) ?
N4 Cu3 Ba1 . 3 126.1(3) ?
Ba3 Cu3 Ba1 3_655 3 70.75(2) ?
Ba3 Cu3 Ba1 2_655 3 110.54(2) ?
Ba3 Cu3 Ba1 4_455 3 69.46(2) ?
Ba3 Cu3 Ba1 1_455 3 109.25(2) ?
N4 Cu3 Ba1 3 . 126.1(3) ?
N4 Cu3 Ba1 . . 53.9(3) ?
Ba3 Cu3 Ba1 3_655 . 109.25(2) ?
Ba3 Cu3 Ba1 2_655 . 69.46(2) ?
Ba3 Cu3 Ba1 4_455 . 110.54(2) ?
Ba3 Cu3 Ba1 1_455 . 70.75(2) ?
Ba1 Cu3 Ba1 3 . 180.0 ?
N4 Cu3 Ba1 3 2 53.9(3) ?
N4 Cu3 Ba1 . 2 126.1(3) ?
Ba3 Cu3 Ba1 3_655 2 110.54(2) ?
Ba3 Cu3 Ba1 2_655 2 70.75(2) ?
Ba3 Cu3 Ba1 4_455 2 109.25(2) ?
Ba3 Cu3 Ba1 1_455 2 69.46(2) ?
Ba1 Cu3 Ba1 3 2 67.61(2) ?
Ba1 Cu3 Ba1 . 2 112.39(2) ?
N4 Cu3 Ba1 3 4 126.1(3) ?
N4 Cu3 Ba1 . 4 53.9(3) ?
Ba3 Cu3 Ba1 3_655 4 69.46(2) ?
Ba3 Cu3 Ba1 2_655 4 109.25(2) ?
Ba3 Cu3 Ba1 4_455 4 70.75(2) ?
Ba3 Cu3 Ba1 1_455 4 110.54(2) ?
Ba1 Cu3 Ba1 3 4 112.39(2) ?
Ba1 Cu3 Ba1 . 4 67.61(2) ?
Ba1 Cu3 Ba1 2 4 180.0 ?
Cu1 N1 Ba7 . . 93.3(3) ?
Cu1 N1 Ba5 . . 88.8(3) ?
Ba7 N1 Ba5 . . 177.6(3) ?
Cu1 N1 Ba4 . . 92.8(3) ?
Ba7 N1 Ba4 . . 93.7(3) ?
Ba5 N1 Ba4 . . 85.1(2) ?
Cu1 N1 Ba10 . . 175.5(4) ?
Ba7 N1 Ba10 . . 89.3(2) ?
Ba5 N1 Ba10 . . 88.7(2) ?
Ba4 N1 Ba10 . . 90.7(2) ?
Cu1 N1 Ba8 . . 89.0(3) ?
Ba7 N1 Ba8 . . 88.9(2) ?
Ba5 N1 Ba8 . . 92.2(2) ?
Ba4 N1 Ba8 . . 176.7(3) ?
Ba10 N1 Ba8 . . 87.4(2) ?
Cu1 N1 In1 . . 68.4(2) ?
Ba7 N1 In1 . . 135.6(2) ?
Ba5 N1 In1 . . 46.40(12) ?
Ba4 N1 In1 . . 126.0(2) ?
Ba10 N1 In1 . . 107.3(2) ?
Ba8 N1 In1 . . 52.34(13) ?
Cu1 N1 In1 . 2_556 67.3(2) ?
Ba7 N1 In1 . 2_556 56.10(15) ?
Ba5 N1 In1 . 2_556 124.0(2) ?
Ba4 N1 In1 . 2_556 49.02(13) ?
Ba10 N1 In1 . 2_556 117.2(2) ?
Ba8 N1 In1 . 2_556 134.3(2) ?
In1 N1 In1 . 2_556 134.73(15) ?
Cu2 N2 Ba3 . 2_655 89.2(4) ?
Cu2 N2 Ba3 . 3_665 89.2(4) ?
Ba3 N2 Ba3 2_655 3_665 94.3(4) ?
Cu2 N2 Ba11 . . 173.6(6) ?
Ba3 N2 Ba11 2_655 . 86.5(3) ?
Ba3 N2 Ba11 3_665 . 86.5(3) ?
Cu2 N2 Ba1 . 4_565 93.0(3) ?
Ba3 N2 Ba1 2_655 4_565 177.4(4) ?
Ba3 N2 Ba1 3_665 4_565 87.21(3) ?
Ba11 N2 Ba1 . 4_565 91.5(3) ?
Cu2 N2 Ba1 . . 93.0(3) ?
Ba3 N2 Ba1 2_655 . 87.21(3) ?
Ba3 N2 Ba1 3_665 . 177.4(4) ?
Ba11 N2 Ba1 . . 91.5(3) ?
Ba1 N2 Ba1 4_565 . 91.2(3) ?
Cu2 N2 In3 . 3_665 114.4(5) ?
Ba3 N2 In3 2_655 3_665 52.20(19) ?
Ba3 N2 In3 3_665 3_665 52.20(19) ?
Ba11 N2 In3 . 3_665 59.2(2) ?
Ba1 N2 In3 4_565 3_665 127.90(19) ?
Ba1 N2 In3 . 3_665 127.90(19) ?
Cu2 N2 In2 . 3_565 69.6(3) ?
Ba3 N2 In2 2_655 3_565 50.0(2) ?
Ba3 N2 In2 3_665 3_565 50.0(2) ?
Ba11 N2 In2 . 3_565 103.9(3) ?
Ba1 N2 In2 4_565 3_565 132.23(19) ?
Ba1 N2 In2 . 3_565 132.23(19) ?
In3 N2 In2 3_665 3_565 44.79(11) ?
Cu2 N2 In2 . . 66.0(3) ?
Ba3 N2 In2 2_655 . 127.9(2) ?
Ba3 N2 In2 3_665 . 127.9(2) ?
Ba11 N2 In2 . . 120.5(3) ?
Ba1 N2 In2 4_565 . 51.95(18) ?
Ba1 N2 In2 . . 51.95(18) ?
In3 N2 In2 3_665 . 179.6(3) ?
In2 N2 In2 3_565 . 135.6(2) ?
Cu2 N2 In3 . . 133.0(5) ?
Ba3 N2 In3 2_655 . 120.5(2) ?
Ba3 N2 In3 3_665 . 120.5(2) ?
Ba11 N2 In3 . . 53.5(2) ?
Ba1 N2 In3 4_565 . 56.9(2) ?
Ba1 N2 In3 . . 56.9(2) ?
In3 N2 In3 3_665 . 112.6(2) ?
In2 N2 In3 3_565 . 157.4(2) ?
In2 N2 In3 . . 67.00(15) ?
Ba5 N3 Ba4 3_666 . 167.1(6) ?
Ba5 N3 Ba2 3_666 . 92.7(3) ?
Ba4 N3 Ba2 . . 96.4(4) ?
Ba5 N3 Ba2 3_666 4_565 92.7(3) ?
Ba4 N3 Ba2 . 4_565 96.4(4) ?
Ba2 N3 Ba2 . 4_565 90.4(4) ?
Ba5 N3 Ba10 3_666 3_666 84.7(3) ?
Ba4 N3 Ba10 . 3_666 86.0(3) ?
Ba2 N3 Ba10 . 3_666 177.1(5) ?
Ba2 N3 Ba10 4_565 3_666 90.85(3) ?
Ba5 N3 Ba10 3_666 . 84.7(3) ?
Ba4 N3 Ba10 . . 86.0(3) ?
Ba2 N3 Ba10 . . 90.85(3) ?
Ba2 N3 Ba10 4_565 . 177.1(5) ?
Ba10 N3 Ba10 3_666 . 87.8(4) ?
Ba5 N3 In2 3_666 . 135.8(4) ?
Ba4 N3 In2 . . 57.1(3) ?
Ba2 N3 In2 . . 58.4(3) ?
Ba2 N3 In2 4_565 . 58.4(3) ?
Ba10 N3 In2 3_666 . 124.4(3) ?
Ba10 N3 In2 . . 124.4(3) ?
Ba5 N3 In3 3_666 . 65.6(2) ?
Ba4 N3 In3 . . 127.2(4) ?
Ba2 N3 In3 . . 51.6(2) ?
Ba2 N3 In3 4_565 . 51.6(2) ?
Ba10 N3 In3 3_666 . 127.8(2) ?
Ba10 N3 In3 . . 127.8(2) ?
In2 N3 In3 . . 70.2(2) ?
Cu3 N4 Ba6 . . 178.6(6) ?
Cu3 N4 Ba3 . 4_455 88.5(4) ?
Ba6 N4 Ba3 . 4_455 92.4(3) ?
Cu3 N4 Ba3 . 1_455 88.5(4) ?
Ba6 N4 Ba3 . 1_455 92.4(3) ?
Ba3 N4 Ba3 4_455 1_455 94.0(4) ?
Cu3 N4 Ba1 . . 93.3(3) ?
Ba6 N4 Ba1 . . 85.7(3) ?
Ba3 N4 Ba1 4_455 . 176.1(4) ?
Ba3 N4 Ba1 1_455 . 89.54(3) ?
Cu3 N4 Ba1 . 4 93.3(3) ?
Ba6 N4 Ba1 . 4 85.7(3) ?
Ba3 N4 Ba1 4_455 4 89.54(3) ?
Ba3 N4 Ba1 1_455 4 176.1(4) ?
Ba1 N4 Ba1 . 4 86.9(3) ?
Cu3 N4 In2 . . 124.69(12) ?
Ba6 N4 In2 . . 55.40(12) ?
Ba3 N4 In2 4_455 . 125.7(3) ?
Ba3 N4 In2 1_455 . 51.89(12) ?
Ba1 N4 In2 . . 55.68(11) ?
Ba1 N4 In2 4 . 124.4(3) ?
Cu3 N4 In2 . 1_545 124.69(12) ?
Ba6 N4 In2 . 1_545 55.40(12) ?
Ba3 N4 In2 4_455 1_545 51.89(12) ?
Ba3 N4 In2 1_455 1_545 125.7(3) ?
Ba1 N4 In2 . 1_545 124.4(3) ?
Ba1 N4 In2 4 1_545 55.68(11) ?
In2 N4 In2 . 1_545 110.4(2) ?
Ba9 N5 Ba6 . . 170.0(6) ?
Ba9 N5 Ba2 . . 95.1(3) ?
Ba6 N5 Ba2 . . 92.0(3) ?
Ba9 N5 Ba2 . 4 95.1(3) ?
Ba6 N5 Ba2 . 4 92.0(3) ?
Ba2 N5 Ba2 . 4 89.1(4) ?
Ba9 N5 Ba1 . 4 90.5(3) ?
Ba6 N5 Ba1 . 4 82.0(3) ?
Ba2 N5 Ba1 . 4 172.8(4) ?
Ba2 N5 Ba1 4 4 94.94(4) ?
Ba9 N5 Ba1 . . 90.5(3) ?
Ba6 N5 Ba1 . . 82.0(3) ?
Ba2 N5 Ba1 . . 94.94(4) ?
Ba2 N5 Ba1 4 . 172.8(4) ?
Ba1 N5 Ba1 4 . 80.4(3) ?
Ba9 N5 In3 . . 55.62(11) ?
Ba6 N5 In3 . . 124.48(11) ?
Ba2 N5 In3 . . 55.36(11) ?
Ba2 N5 In3 4 . 125.9(4) ?
Ba1 N5 In3 4 . 125.4(3) ?
Ba1 N5 In3 . . 61.10(10) ?
Ba9 N5 In3 . 1_545 55.62(11) ?
Ba6 N5 In3 . 1_545 124.48(11) ?
Ba2 N5 In3 . 1_545 125.9(4) ?
Ba2 N5 In3 4 1_545 55.36(11) ?
Ba1 N5 In3 4 1_545 61.10(10) ?
Ba1 N5 In3 . 1_545 125.4(3) ?
In3 N5 In3 . 1_545 110.8(2) ?
Ba9 N5 In2 . 1_545 125.58(11) ?
Ba6 N5 In2 . 1_545 54.22(10) ?
Ba2 N5 In2 . 1_545 124.4(3) ?
Ba2 N5 In2 4 1_545 55.08(11) ?
Ba1 N5 In2 4 1_545 54.59(10) ?
Ba1 N5 In2 . 1_545 117.9(3) ?
In3 N5 In2 . 1_545 178.6(2) ?
In3 N5 In2 1_545 1_545 70.43(2) ?
Ba9 N5 In2 . . 125.58(11) ?
Ba6 N5 In2 . . 54.22(10) ?
Ba2 N5 In2 . . 55.08(11) ?
Ba2 N5 In2 4 . 124.4(3) ?
Ba1 N5 In2 4 . 117.9(3) ?
Ba1 N5 In2 . . 54.59(10) ?
In3 N5 In2 . . 70.43(2) ?
In3 N5 In2 1_545 . 178.6(2) ?
In2 N5 In2 1_545 . 108.3(2) ?
Ba9 N5 In1 . 2_656 40.43(17) ?
Ba6 N5 In1 . 2_656 146.1(2) ?
Ba2 N5 In1 . 2_656 54.63(18) ?
Ba2 N5 In1 4 2_656 93.3(3) ?
Ba1 N5 In1 4 2_656 130.8(3) ?
Ba1 N5 In1 . 2_656 93.89(17) ?
In3 N5 In1 . 2_656 33.96(7) ?
In3 N5 In1 1_545 2_656 85.21(18) ?
In2 N5 In1 1_545 2_656 147.3(2) ?
In2 N5 In1 . 2_656 96.14(8) ?
Ba9 N5 In1 . 3_656 40.43(17) ?
Ba6 N5 In1 . 3_656 146.1(2) ?
Ba2 N5 In1 . 3_656 93.3(3) ?
Ba2 N5 In1 4 3_656 54.63(18) ?
Ba1 N5 In1 4 3_656 93.89(17) ?
Ba1 N5 In1 . 3_656 130.8(3) ?
In3 N5 In1 . 3_656 85.21(18) ?
In3 N5 In1 1_545 3_656 33.96(7) ?
In2 N5 In1 1_545 3_656 96.14(8) ?
In2 N5 In1 . 3_656 147.3(2) ?
In1 N5 In1 2_656 3_656 53.88(12) ?
Ba2 N6 Ba2 4 . 95.4(4) ?
Ba2 N6 Ba8 4 3_656 93.8(4) ?
Ba2 N6 Ba8 . 3_656 93.8(4) ?
Ba2 N6 Ba7 4 . 99.6(4) ?
Ba2 N6 Ba7 . . 99.6(4) ?
Ba8 N6 Ba7 3_656 . 160.0(5) ?
Ba2 N6 Ba10 4 . 170.2(4) ?
Ba2 N6 Ba10 . . 93.88(7) ?
Ba8 N6 Ba10 3_656 . 82.2(3) ?
Ba7 N6 Ba10 . . 82.1(3) ?
Ba2 N6 Ba10 4 3_656 93.88(7) ?
Ba2 N6 Ba10 . 3_656 170.2(4) ?
Ba8 N6 Ba10 3_656 3_656 82.2(3) ?
Ba7 N6 Ba10 . 3_656 82.1(3) ?
Ba10 N6 Ba10 . 3_656 76.7(3) ?
loop_
_geom_bond_atom_site_label_1
_geom_bond_atom_site_label_2
_geom_bond_site_symmetry_2
_geom_bond_distance
_geom_bond_publ_flag
Ba1 N4 . 2.810(9) yes
Ba1 N2 . 2.901(9) yes
Ba1 N5 . 2.993(10) yes
Ba2 N6 . 2.662(9) yes
Ba2 N5 . 2.805(9) yes
Ba2 N3 . 2.869(10) yes
Ba3 N2 3_665 2.701(8) yes
Ba3 N4 1_655 2.768(8) yes
Ba4 N3 . 2.750(12) yes
Ba4 N1 4_565 2.773(8) yes
Ba4 N1 . 2.773(8) yes
Ba5 N3 3_666 2.719(13) yes
Ba5 N1 . 2.773(8) yes
Ba5 N1 4_565 2.773(8) yes
Ba6 N4 . 2.582(12) yes
Ba6 N5 . 2.586(11) yes
Ba7 N1 . 2.715(8) yes
Ba7 N1 4 2.715(8) yes
Ba7 N6 . 2.792(15) yes
Ba8 N6 3_656 2.762(15) yes
Ba8 N1 4 2.787(8) yes
Ba8 N1 . 2.787(8) yes
Ba9 N5 . 2.466(11) yes
Ba10 N1 2_656 2.775(7) yes
Ba10 N1 . 2.775(7) yes
Ba10 N3 3_666 3.026(11) yes
Ba10 N3 . 3.026(10) yes
Ba10 N6 . 3.074(11) yes
Ba10 N6 3_656 3.074(11) yes
Ba11 N2 . 2.762(10) yes
Ba11 N2 3_665 2.762(10) yes
Ba12 Ba3 3_655 3.7654(8) yes
Ba12 Ba3 . 3.7654(8) yes
Ba12 Ba3 2_655 3.7654(8) yes
Ba12 Ba3 4 3.7654(8) yes
Ba12 Ba9 3_655 3.8978(13) yes
Ba12 Ba9 . 3.8978(13) yes
Ba12 Ba1 3_655 3.9894(8) yes
Ba12 Ba1 2_655 3.9894(8) yes
Ba12 Ba1 . 3.9894(8) yes
Ba12 Ba1 4 3.9894(8) yes
Ba12 Ba11 . 4.0045(8) yes
Ba12 Ba11 1_545 4.0045(8) yes
In1 In3 3_666 2.9548(14) yes
In1 In2 3_566 2.9632(12) yes
In1 In1 4_565 3.3009(16) yes
In2 In3 1_455 3.7310(17) yes
Cu1 N1 2_556 1.890(7) yes
Cu1 N1 . 1.890(7) yes
Cu2 N2 3_565 1.906(10) yes
Cu2 N2 . 1.906(10) yes
Cu3 N4 3 1.886(12) yes
Cu3 N4 . 1.886(12) yes
Cu3 Ba3 3_655 3.3092(7) ?
Cu3 Ba3 2_655 3.3092(7) ?
Cu3 Ba3 4_455 3.3092(7) ?
Cu3 Ba3 1_455 3.3092(7) ?
Cu3 Ba1 3 3.4729(8) ?
Cu3 Ba1 2 3.4729(8) ?
Cu3 Ba1 4 3.4729(8) ?
N1 In1 2_556 5.035(8) ?
N2 Ba3 2_655 2.701(8) ?
N2 Ba3 3_665 2.701(8) ?
N2 Ba1 4_565 2.901(9) ?
N2 In3 3_665 4.810(11) ?
N2 In2 3_565 4.976(12) ?
N3 Ba5 3_666 2.719(13) ?
N3 Ba2 4_565 2.869(10) ?
N3 Ba10 3_666 3.026(11) ?
N4 Ba3 4_455 2.768(8) ?
N4 Ba3 1_455 2.768(8) ?
N4 Ba1 4 2.810(9) ?
N4 In2 1_545 4.878(7) ?
N5 Ba2 4 2.805(9) ?
N5 Ba1 4 2.993(10) ?
N5 In3 1_545 4.864(6) ?
N5 In2 1_545 4.941(7) ?
N5 In1 2_656 5.196(11) ?
N5 In1 3_656 5.196(11) ?
N6 Ba2 4 2.662(9) ?
N6 Ba8 3_656 2.762(15) ?
N6 Ba10 3_656 3.074(11) ?
